# Supplementary Information (SI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2025

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_heka_0015_sq
_database_code_depnum_ccdc_archive 'CCDC 2341647'
loop_
_audit_author_name
_audit_author_address
'Robert Gyepes'
;Department of Inorganic Chemistry, Charles University, Prague
Czech Republic
;
_audit_update_record             
;
2024-10-03 deposited with the CCDC.	2024-12-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2019/2
_shelx_SHELXL_version_number     2019/2
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'H52 La6 O92 V23, 24[H2O]'
_chemical_formula_sum            'H100 La6 O116 V23'
_chemical_formula_weight         3961.87

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.2130(10)
_cell_length_b                   20.8813(16)
_cell_length_c                   18.7007(14)
_cell_angle_alpha                90
_cell_angle_beta                 97.169(2)
_cell_angle_gamma                90
_cell_volume                     5119.3(7)
_cell_formula_units_Z            2
_cell_measurement_temperature    120(2)
_cell_measurement_reflns_used    9525
_cell_measurement_theta_min      2.4020
_cell_measurement_theta_max      27.1280

_exptl_crystal_description       plate
_exptl_crystal_colour            'translucent yellow'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.570
_exptl_crystal_F_000             3798
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.549
_exptl_crystal_size_mid          0.523
_exptl_crystal_size_min          0.080
_exptl_absorpt_coefficient_mu    4.564
_shelx_estimated_absorpt_T_min   0.188
_shelx_estimated_absorpt_T_max   0.712
_exptl_absorpt_correction_type   'Numerical Mu From Formula'
_exptl_absorpt_process_details   
;
Krause, L., Herbst-Irmer, R., Sheldrick, G. M., Stalke, D. (2015).
"Comparison of silver and molybdenum microfocus X-ray sources for
single-crystal structure determination"
J. Appl. Cryst. 48, 3-10.
doi:10.1107/S1600576714022985
;
_exptl_absorpt_correction_T_min  0.21
_exptl_absorpt_correction_T_max  0.68
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      120(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device       'κ-geometry diffractometer'
_diffrn_measurement_device_type  'Bruker Nonius Kappa APEX II'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            120234
_diffrn_reflns_av_unetI/netI     0.0359
_diffrn_reflns_av_R_equivalents  0.0838
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_theta_min         1.951
_diffrn_reflns_theta_max         25.999
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             10062
_reflns_number_gt                8407
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2019/2 (Sheldrick, 2019)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0317P)²+35.9953P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   difmap
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         10062
_refine_ls_number_parameters     625
_refine_ls_number_restraints     40
_refine_ls_R_factor_all          0.0490
_refine_ls_R_factor_gt           0.0363
_refine_ls_wR_factor_ref         0.0849
_refine_ls_wR_factor_gt          0.0809
_refine_ls_goodness_of_fit_ref   1.075
_refine_ls_restrained_S_all      1.080
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.76163(2) 0.56157(2) 0.73163(2) 0.01075(8) Uani 1 1 d . . . . .
La2 La 0.22627(2) 0.42609(2) 0.67570(2) 0.01431(9) Uani 1 1 d . . . . .
La3 La 0.34743(3) 0.74064(2) 0.49503(2) 0.01985(9) Uani 1 1 d . . . . .
V1 V 0.83469(7) 0.50394(5) 0.90116(5) 0.00918(19) Uani 1 1 d . . . . .
V2 V 0.92929(7) 0.47304(5) 1.05969(5) 0.00753(19) Uani 1 1 d . . . . .
V3 V 1.02498(7) 0.61211(5) 1.07339(5) 0.0102(2) Uani 1 1 d . . . . .
V4 V 0.92707(7) 0.64122(5) 0.91736(5) 0.0107(2) Uani 1 1 d . . . . .
V5 V 0.79234(7) 0.59094(5) 1.02778(5) 0.0119(2) Uani 1 1 d . . . . .
V6 V 0.54862(7) 0.62458(5) 0.59392(5) 0.00945(19) Uani 1 1 d . . . . .
V7 V 0.72578(7) 0.55585(5) 0.52516(5) 0.00804(19) Uani 1 1 d . . . . .
V8 V 0.67333(7) 0.42663(5) 0.59874(5) 0.00884(19) Uani 1 1 d . . . . .
V9 V 0.49667(7) 0.49493(5) 0.66954(5) 0.00956(19) Uani 1 1 d . . . . .
V10 V 0.32374(7) 0.56786(5) 0.57135(5) 0.00940(19) Uani 1 1 d . . . . .
V11 V 0.500000 0.500000 0.500000 0.0085(3) Uani 1 2 d S . P . .
V12 V 0.44979(7) 0.37128(5) 0.57552(5) 0.0106(2) Uani 1 1 d . . . . .
O1 O 0.8607(3) 0.57905(18) 0.85463(18) 0.0096(8) Uani 1 1 d . . . . .
O2 O 0.7689(3) 0.47023(19) 0.8322(2) 0.0136(8) Uani 1 1 d . . . . .
O3 O 0.7404(3) 0.53646(19) 0.95070(19) 0.0118(8) Uani 1 1 d . . . . .
O4 O 0.8659(3) 0.43432(18) 0.97049(19) 0.0091(8) Uani 1 1 d . . . . .
O5 O 1.0601(3) 0.44896(17) 1.01402(18) 0.0080(8) Uani 1 1 d . . . . .
O6 O 0.9439(3) 0.40594(18) 1.10830(19) 0.0111(8) Uani 1 1 d . . . . .
O7 O 0.8216(3) 0.50947(19) 1.08207(19) 0.0117(8) Uani 1 1 d . . . . .
O8 O 1.0240(3) 0.52590(18) 1.11758(18) 0.0092(8) Uani 1 1 d . . . . .
O9 O 0.6910(3) 0.6133(2) 1.0580(2) 0.0211(10) Uani 1 1 d . . . . .
O10 O 0.8946(3) 0.62554(19) 1.09452(19) 0.0126(8) Uani 1 1 d . . . . .
O11 O 1.0933(3) 0.6507(2) 1.1357(2) 0.0177(9) Uani 1 1 d . . . . .
O12 O 1.0135(3) 0.66858(18) 0.99740(19) 0.0112(8) Uani 1 1 d . . . . .
O13 O 0.8131(3) 0.65403(19) 0.96028(19) 0.0126(8) Uani 1 1 d . . . . .
O14 O 0.9316(3) 0.7009(2) 0.8632(2) 0.0164(9) Uani 1 1 d . . . . .
O15 O 0.6687(4) 0.6300(3) 0.8193(2) 0.0321(12) Uani 1 1 d D . . . .
H15A H 0.645(6) 0.667(2) 0.814(5) 0.048 Uiso 1 1 d D U . . .
H15B H 0.698(6) 0.633(4) 0.860(2) 0.048 Uiso 1 1 d D U . . .
O16 O 0.8611(4) 0.6634(2) 0.7211(3) 0.0264(11) Uani 1 1 d . . . . .
H16A H 0.878(7) 0.683(4) 0.752(5) 0.040 Uiso 1 1 d . U . . .
H16B H 0.842(6) 0.700(4) 0.703(4) 0.040 Uiso 1 1 d . U . . .
O17 O 0.9410(3) 0.5171(2) 0.7391(2) 0.0194(9) Uani 1 1 d D . . . .
H17A H 0.983(4) 0.504(3) 0.715(3) 0.029 Uiso 1 1 d D U . . .
H17B H 0.963(5) 0.505(3) 0.779(2) 0.029 Uiso 1 1 d D U . . .
O18 O 0.6355(3) 0.63563(19) 0.66355(19) 0.0117(8) Uani 1 1 d . . . . .
O19 O 0.7978(3) 0.57195(19) 0.60211(18) 0.0106(8) Uani 1 1 d . . . . .
O20 O 0.7494(3) 0.45343(19) 0.66903(19) 0.0118(8) Uani 1 1 d . . . . .
O21 O 0.5877(3) 0.5159(2) 0.73383(19) 0.0138(9) Uani 1 1 d . . . . .
O22 O 0.4457(3) 0.57881(18) 0.63922(18) 0.0097(8) Uani 1 1 d . . . . .
O23 O 0.5506(3) 0.41329(18) 0.64342(19) 0.0103(8) Uani 1 1 d . . . . .
O24 O 0.7398(3) 0.46354(18) 0.52161(19) 0.0088(8) Uani 1 1 d . . . . .
O25 O 0.5976(3) 0.52241(18) 0.58327(18) 0.0092(8) Uani 1 1 d . . . . .
O26 O 0.7962(3) 0.57473(18) 0.46201(19) 0.0098(8) Uani 1 1 d . . . . .
O27 O 0.7086(3) 0.35177(19) 0.5900(2) 0.0128(8) Uani 1 1 d . . . . .
O28 O 0.5530(3) 0.41579(18) 0.50251(18) 0.0097(8) Uani 1 1 d . U . . .
O29 O 0.4029(3) 0.47461(19) 0.56312(19) 0.0109(8) Uani 1 1 d . . . . .
O30 O 0.3646(3) 0.37065(18) 0.48249(19) 0.0099(8) Uani 1 1 d . . . . .
O31 O 0.2457(3) 0.5371(2) 0.62411(19) 0.0132(8) Uani 1 1 d . . . . .
O32 O 0.3600(3) 0.3582(2) 0.6276(2) 0.0153(9) Uani 1 1 d . . . . .
O33 O 0.4026(3) 0.4704(2) 0.71305(19) 0.0153(9) Uani 1 1 d . . . . .
O34 O 0.1312(4) 0.3294(2) 0.6221(3) 0.0274(11) Uani 1 1 d D . . . .
H34A H 0.136(6) 0.324(4) 0.5800(19) 0.041 Uiso 1 1 d D U . . .
H34B H 0.108(6) 0.298(3) 0.641(4) 0.041 Uiso 1 1 d D U . . .
O35 O 0.0472(3) 0.4701(3) 0.6296(2) 0.0200(10) Uani 1 1 d . . . . .
H35A H 0.049(6) 0.510(4) 0.617(4) 0.030 Uiso 1 1 d . U . . .
H35B H 0.006(6) 0.454(4) 0.600(4) 0.030 Uiso 1 1 d . U . . .
O36 O 0.0970(4) 0.3858(3) 0.7558(2) 0.0338(12) Uani 1 1 d D U . . .
H36A H 0.038(3) 0.376(4) 0.743(5) 0.051 Uiso 1 1 d D U . . .
H36B H 0.095(6) 0.376(4) 0.798(2) 0.051 Uiso 1 1 d D U . . .
O37 O 0.3125(5) 0.3590(4) 0.7784(4) 0.068(2) Uani 1 1 d D . . . .
H37A H 0.277(8) 0.331(4) 0.795(6) 0.102 Uiso 1 1 d D U . . .
H37B H 0.381701 0.359(6) 0.795(5) 0.102 Uiso 1 1 d D U . . .
O38 O 0.2119(5) 0.5097(3) 0.7729(3) 0.0421(14) Uani 1 1 d D . . . .
H38A H 0.197(7) 0.505(5) 0.813(2) 0.063 Uiso 1 1 d D U . . .
H38B H 0.203(8) 0.5487(18) 0.766(5) 0.063 Uiso 1 1 d D U . . .
O39 O 0.4906(3) 0.6939(2) 0.5812(2) 0.0168(9) Uani 1 1 d . . . . .
O40 O 0.4936(4) 0.8194(3) 0.5086(4) 0.0432(15) Uani 1 1 d . . . . .
H40A H 0.482(8) 0.854(5) 0.521(5) 0.065 Uiso 1 1 d . U . . .
H40B H 0.545(8) 0.802(5) 0.498(5) 0.065 Uiso 1 1 d . U . . .
O41A O 0.3214(11) 0.7924(6) 0.3754(7) 0.048(3) Uani 0.65 1 d D U P A 1
H41A H 0.373(5) 0.807(5) 0.360(5) 0.072 Uiso 1 1 d D U . B 1
H41B H 0.275(6) 0.772(5) 0.350(5) 0.072 Uiso 1 1 d D U . C 1
O41B O 0.3262(19) 0.7760(11) 0.3561(13) 0.039(6) Uiso 0.35 1 d . . P A 2
O42 O 0.1534(3) 0.7369(2) 0.4714(3) 0.0306(11) Uani 1 1 d D . . . .
H42A H 0.120(6) 0.704(3) 0.461(4) 0.046 Uiso 1 1 d D U . . .
H42B H 0.110(5) 0.763(3) 0.480(4) 0.046 Uiso 1 1 d D U . . .
O43 O 0.2885(3) 0.64323(19) 0.5610(2) 0.0144(8) Uani 1 1 d . . . . .
O44 O 0.5066(3) 0.3018(2) 0.5704(2) 0.0159(9) Uani 1 1 d . . . . .
O45 O 0.3158(7) 0.7706(4) 0.6141(4) 0.093(3) Uani 1 1 d . U . . .
O46A O 0.2952(9) 0.8548(6) 0.5194(8) 0.036(3) Uani 0.5 1 d . . P A 1
O46B O 0.2781(9) 0.8556(6) 0.4746(7) 0.034(3) Uani 0.5 1 d . . P A 2


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 O21 2.493(4) . ?
La1 O18 2.502(4) . ?
La1 O16 2.520(5) . ?
La1 O1 2.527(3) . ?
La1 O17 2.533(4) . ?
La1 O19 2.536(3) . ?
La1 O20 2.539(4) . ?
La1 O15 2.596(4) . ?
La1 O2 2.672(4) . ?
La1 V1 3.4158(9) . ?
La2 O32 2.518(4) . ?
La2 O34 2.520(5) . ?
La2 O33 2.523(4) . ?
La2 O37 2.531(6) . ?
La2 O31 2.536(4) . ?
La2 O38 2.545(5) . ?
La2 O36 2.551(4) . ?
La2 O26 2.555(3) 3_666 ?
La2 O35 2.584(4) . ?
La3 O45 2.399(7) . ?
La3 O41A 2.470(11) . ?
La3 O39 2.523(4) . ?
La3 O40 2.525(5) . ?
La3 O46A 2.539(12) . ?
La3 O42 2.548(5) . ?
La3 O43 2.550(4) . ?
La3 O27 2.551(4) 3_666 ?
La3 O44 2.567(4) 3_666 ?
La3 O46B 2.581(12) . ?
La3 O41B 2.68(2) . ?
V1 O2 1.623(4) . ?
V1 O3 1.778(4) . ?
V1 O1 1.847(4) . ?
V1 O4 1.957(4) . ?
V1 O8 2.039(4) 3_767 ?
V1 O5 2.206(4) 3_767 ?
V1 V3 3.0523(14) 3_767 ?
V1 V5 3.0906(13) . ?
V1 V4 3.1155(14) . ?
V2 O6 1.668(4) . ?
V2 O7 1.711(4) . ?
V2 O8 1.902(4) . ?
V2 O4 1.947(4) . ?
V2 O5 2.083(4) . ?
V2 O5 2.150(4) 3_767 ?
V2 V4 3.0456(13) 3_767 ?
V2 V5 3.0696(13) . ?
V3 O11 1.599(4) . ?
V3 O10 1.836(4) . ?
V3 O12 1.838(4) . ?
V3 O8 1.982(4) . ?
V3 O4 1.997(4) 3_767 ?
V3 O5 2.259(4) 3_767 ?
V3 V4 3.1009(13) . ?
V3 V5 3.1173(13) . ?
V4 O14 1.612(4) . ?
V4 O13 1.813(4) . ?
V4 O12 1.856(4) . ?
V4 O1 1.890(4) . ?
V4 O6 2.077(4) 3_767 ?
V4 O5 2.273(4) 3_767 ?
V4 V5 3.0747(13) . ?
V5 O9 1.587(4) . ?
V5 O10 1.867(4) . ?
V5 O13 1.868(4) . ?
V5 O3 1.897(4) . ?
V5 O7 1.994(4) . ?
V5 O5 2.342(4) 3_767 ?
V6 O39 1.641(4) . ?
V6 O18 1.641(4) . ?
V6 O22 1.941(4) . ?
V6 O30 1.943(4) 3_666 ?
V6 O25 2.245(4) . ?
V6 O28 2.272(4) 3_666 ?
V7 O26 1.640(4) . ?
V7 O19 1.658(4) . ?
V7 O24 1.938(4) . ?
V7 O30 1.939(4) 3_666 ?
V7 O25 2.235(4) . ?
V7 O29 2.306(4) 3_666 ?
V8 O27 1.645(4) . ?
V8 O20 1.650(4) . ?
V8 O23 1.935(4) . ?
V8 O24 1.939(4) . ?
V8 O25 2.239(4) . ?
V8 O28 2.259(4) . ?
V9 O33 1.650(4) . ?
V9 O21 1.650(4) . ?
V9 O23 1.934(4) . ?
V9 O22 1.936(4) . ?
V9 O29 2.250(4) . ?
V9 O25 2.290(4) . ?
V10 O31 1.645(4) . ?
V10 O43 1.646(4) . ?
V10 O22 1.936(4) . ?
V10 O24 1.948(4) 3_666 ?
V10 O29 2.224(4) . ?
V10 O28 2.289(4) 3_666 ?
V11 O28 1.891(4) 3_666 ?
V11 O28 1.891(4) . ?
V11 O29 1.924(4) 3_666 ?
V11 O29 1.924(4) . ?
V11 O25 1.951(3) . ?
V11 O25 1.951(3) 3_666 ?
V12 O44 1.642(4) . ?
V12 O32 1.649(4) . ?
V12 O23 1.932(4) . ?
V12 O30 1.950(4) . ?
V12 O28 2.248(4) . ?
V12 O29 2.249(4) . ?
O15 H15A 0.83(3) . ?
O15 H15B 0.81(3) . ?
O16 H16A 0.72(9) . ?
O16 H16B 0.86(9) . ?
O17 H17A 0.80(3) . ?
O17 H17B 0.80(3) . ?
O34 H34A 0.81(3) . ?
O34 H34B 0.81(3) . ?
O35 H35A 0.86(8) . ?
O35 H35B 0.80(8) . ?
O36 H36A 0.82(3) . ?
O36 H36B 0.82(3) . ?
O37 H37A 0.83(3) . ?
O37 H37B 0.93(2) . ?
O38 H38A 0.81(3) . ?
O38 H38B 0.83(3) . ?
O40 H40A 0.79(10) . ?
O40 H40B 0.82(10) . ?
O41A H41A 0.83(3) . ?
O41A H41B 0.85(3) . ?
O42 H42A 0.83(3) . ?
O42 H42B 0.83(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O21 La1 O18 71.83(13) . . ?
O21 La1 O16 144.55(15) . . ?
O18 La1 O16 76.08(15) . . ?
O21 La1 O1 114.47(12) . . ?
O18 La1 O1 127.62(12) . . ?
O16 La1 O1 74.52(14) . . ?
O21 La1 O17 135.81(14) . . ?
O18 La1 O17 144.45(13) . . ?
O16 La1 O17 79.63(16) . . ?
O1 La1 O17 68.15(12) . . ?
O21 La1 O19 109.43(12) . . ?
O18 La1 O19 69.77(12) . . ?
O16 La1 O19 72.01(14) . . ?
O1 La1 O19 135.96(12) . . ?
O17 La1 O19 78.29(12) . . ?
O21 La1 O20 70.24(12) . . ?
O18 La1 O20 108.37(12) . . ?
O16 La1 O20 135.90(14) . . ?
O1 La1 O20 122.94(12) . . ?
O17 La1 O20 72.82(13) . . ?
O19 La1 O20 69.17(12) . . ?
O21 La1 O15 71.98(16) . . ?
O18 La1 O15 69.12(13) . . ?
O16 La1 O15 82.92(18) . . ?
O1 La1 O15 65.04(13) . . ?
O17 La1 O15 132.85(14) . . ?
O19 La1 O15 135.76(14) . . ?
O20 La1 O15 140.62(16) . . ?
O21 La1 O2 70.58(12) . . ?
O18 La1 O2 139.69(12) . . ?
O16 La1 O2 133.14(13) . . ?
O1 La1 O2 59.56(12) . . ?
O17 La1 O2 75.44(13) . . ?
O19 La1 O2 137.63(12) . . ?
O20 La1 O2 71.60(12) . . ?
O15 La1 O2 85.81(15) . . ?
O21 La1 V1 90.24(8) . . ?
O18 La1 V1 141.56(8) . . ?
O16 La1 V1 106.25(11) . . ?
O1 La1 V1 31.98(9) . . ?
O17 La1 V1 70.47(9) . . ?
O19 La1 V1 148.36(8) . . ?
O20 La1 V1 96.25(8) . . ?
O15 La1 V1 73.09(11) . . ?
O2 La1 V1 27.62(8) . . ?
O32 La2 O34 75.16(15) . . ?
O32 La2 O33 68.90(13) . . ?
O34 La2 O33 143.25(15) . . ?
O32 La2 O37 71.9(2) . . ?
O34 La2 O37 90.7(2) . . ?
O33 La2 O37 71.35(18) . . ?
O32 La2 O31 105.67(12) . . ?
O34 La2 O31 130.58(14) . . ?
O33 La2 O31 68.70(12) . . ?
O37 La2 O31 137.5(2) . . ?
O32 La2 O38 139.44(17) . . ?
O34 La2 O38 139.13(17) . . ?
O33 La2 O38 72.51(17) . . ?
O37 La2 O38 84.5(3) . . ?
O31 La2 O38 70.43(15) . . ?
O32 La2 O36 125.11(16) . . ?
O34 La2 O36 68.41(17) . . ?
O33 La2 O36 128.39(14) . . ?
O37 La2 O36 69.04(18) . . ?
O31 La2 O36 129.18(16) . . ?
O38 La2 O36 72.03(18) . . ?
O32 La2 O26 68.58(12) . 3_666 ?
O34 La2 O26 66.70(14) . 3_666 ?
O33 La2 O26 105.58(12) . 3_666 ?
O37 La2 O26 138.2(2) . 3_666 ?
O31 La2 O26 68.11(12) . 3_666 ?
O38 La2 O26 135.65(16) . 3_666 ?
O36 La2 O26 125.99(14) . 3_666 ?
O32 La2 O35 137.34(13) . . ?
O34 La2 O35 76.24(17) . . ?
O33 La2 O35 137.52(15) . . ?
O37 La2 O35 139.19(17) . . ?
O31 La2 O35 71.31(14) . . ?
O38 La2 O35 81.24(18) . . ?
O36 La2 O35 70.20(15) . . ?
O26 La2 O35 71.31(12) 3_666 . ?
O45 La3 O41A 134.9(4) . . ?
O45 La3 O39 73.3(2) . . ?
O41A La3 O39 139.1(3) . . ?
O45 La3 O40 87.5(3) . . ?
O41A La3 O40 79.9(4) . . ?
O39 La3 O40 71.62(18) . . ?
O45 La3 O46A 60.4(4) . . ?
O41A La3 O46A 75.0(5) . . ?
O39 La3 O46A 116.6(3) . . ?
O40 La3 O46A 65.9(3) . . ?
O45 La3 O42 83.1(2) . . ?
O41A La3 O42 80.4(4) . . ?
O39 La3 O42 139.18(15) . . ?
O40 La3 O42 141.07(18) . . ?
O46A La3 O42 76.7(3) . . ?
O45 La3 O43 70.1(2) . . ?
O41A La3 O43 140.4(3) . . ?
O39 La3 O43 68.43(13) . . ?
O40 La3 O43 138.30(18) . . ?
O46A La3 O43 123.8(3) . . ?
O42 La3 O43 72.42(15) . . ?
O45 La3 O27 134.8(2) . 3_666 ?
O41A La3 O27 76.7(3) . 3_666 ?
O39 La3 O27 103.98(12) . 3_666 ?
O40 La3 O27 135.57(17) . 3_666 ?
O46A La3 O27 139.3(3) . 3_666 ?
O42 La3 O27 70.20(14) . 3_666 ?
O43 La3 O27 67.40(12) . 3_666 ?
O45 La3 O44 139.5(2) . 3_666 ?
O41A La3 O44 75.4(4) . 3_666 ?
O39 La3 O44 67.83(12) . 3_666 ?
O40 La3 O44 70.27(17) . 3_666 ?
O46A La3 O44 130.3(3) . 3_666 ?
O42 La3 O44 134.93(15) . 3_666 ?
O43 La3 O44 104.33(12) . 3_666 ?
O27 La3 O44 67.57(12) 3_666 3_666 ?
O45 La3 O46B 78.2(4) . . ?
O39 La3 O46B 132.7(3) . . ?
O40 La3 O46B 70.2(3) . . ?
O42 La3 O46B 70.9(3) . . ?
O43 La3 O46B 133.6(3) . . ?
O27 La3 O46B 122.8(3) 3_666 . ?
O44 La3 O46B 121.6(3) 3_666 . ?
O45 La3 O41B 144.9(5) . . ?
O39 La3 O41B 134.8(5) . . ?
O40 La3 O41B 84.5(6) . . ?
O42 La3 O41B 81.9(6) . . ?
O43 La3 O41B 133.4(6) . . ?
O27 La3 O41B 67.5(5) 3_666 . ?
O44 La3 O41B 68.1(5) 3_666 . ?
O46B La3 O41B 66.9(6) . . ?
O2 V1 O3 103.82(19) . . ?
O2 V1 O1 96.14(18) . . ?
O3 V1 O1 96.04(17) . . ?
O2 V1 O4 104.58(18) . . ?
O3 V1 O4 92.41(17) . . ?
O1 V1 O4 155.05(16) . . ?
O2 V1 O8 98.17(17) . 3_767 ?
O3 V1 O8 157.29(16) . 3_767 ?
O1 V1 O8 87.14(16) . 3_767 ?
O4 V1 O8 76.41(15) . 3_767 ?
O2 V1 O5 172.63(17) . 3_767 ?
O3 V1 O5 82.81(15) . 3_767 ?
O1 V1 O5 79.77(15) . 3_767 ?
O4 V1 O5 78.06(14) . 3_767 ?
O8 V1 O5 75.62(14) 3_767 3_767 ?
O2 V1 V3 91.96(15) . 3_767 ?
O3 V1 V3 132.35(13) . 3_767 ?
O1 V1 V3 127.04(12) . 3_767 ?
O4 V1 V3 39.95(11) . 3_767 ?
O8 V1 V3 39.91(11) 3_767 3_767 ?
O5 V1 V3 85.75(10) 3_767 3_767 ?
O2 V1 V5 137.17(14) . . ?
O3 V1 V5 33.95(12) . . ?
O1 V1 V5 85.64(12) . . ?
O4 V1 V5 88.42(11) . . ?
O8 V1 V5 124.64(11) 3_767 . ?
O5 V1 V5 49.08(10) 3_767 . ?
V3 V1 V5 120.78(4) 3_767 . ?
O2 V1 V4 129.86(15) . . ?
O3 V1 V4 83.66(13) . . ?
O1 V1 V4 33.96(11) . . ?
O4 V1 V4 124.84(11) . . ?
O8 V1 V4 86.67(11) 3_767 . ?
O5 V1 V4 46.82(10) 3_767 . ?
V3 V1 V4 119.49(4) 3_767 . ?
V5 V1 V4 59.39(3) . . ?
O2 V1 La1 49.77(14) . . ?
O3 V1 La1 102.35(12) . . ?
O1 V1 La1 46.46(11) . . ?
O4 V1 La1 152.66(11) . . ?
O8 V1 La1 96.14(10) 3_767 . ?
O5 V1 La1 126.16(10) 3_767 . ?
V3 V1 La1 121.35(3) 3_767 . ?
V5 V1 La1 116.54(3) . . ?
V4 V1 La1 80.09(3) . . ?
O6 V2 O7 106.45(18) . . ?
O6 V2 O8 98.87(17) . . ?
O7 V2 O8 96.38(17) . . ?
O6 V2 O4 97.25(17) . . ?
O7 V2 O4 96.45(17) . . ?
O8 V2 O4 155.62(15) . . ?
O6 V2 O5 88.59(16) . . ?
O7 V2 O5 164.94(17) . . ?
O8 V2 O5 81.52(15) . . ?
O4 V2 O5 80.71(14) . . ?
O6 V2 O5 166.78(16) . 3_767 ?
O7 V2 O5 86.71(16) . 3_767 ?
O8 V2 O5 80.47(15) . 3_767 ?
O4 V2 O5 79.67(14) . 3_767 ?
O5 V2 O5 78.24(16) . 3_767 ?
O6 V2 V4 40.33(13) . 3_767 ?
O7 V2 V4 146.78(13) . 3_767 ?
O8 V2 V4 91.15(12) . 3_767 ?
O4 V2 V4 89.39(12) . 3_767 ?
O5 V2 V4 48.26(10) . 3_767 ?
O5 V2 V4 126.48(10) 3_767 3_767 ?
O6 V2 V5 143.59(13) . . ?
O7 V2 V5 37.13(13) . . ?
O8 V2 V5 88.59(12) . . ?
O4 V2 V5 89.22(11) . . ?
O5 V2 V5 127.82(11) . . ?
O5 V2 V5 49.58(10) 3_767 . ?
V4 V2 V5 176.03(4) 3_767 . ?
O11 V3 O10 103.05(19) . . ?
O11 V3 O12 103.0(2) . . ?
O10 V3 O12 94.54(17) . . ?
O11 V3 O8 100.71(19) . . ?
O10 V3 O8 89.66(16) . . ?
O12 V3 O8 154.28(16) . . ?
O11 V3 O4 99.95(19) . 3_767 ?
O10 V3 O4 155.15(17) . 3_767 ?
O12 V3 O4 89.32(16) . 3_767 ?
O8 V3 O4 76.86(15) . 3_767 ?
O11 V3 O5 174.82(18) . 3_767 ?
O10 V3 O5 81.17(15) . 3_767 ?
O12 V3 O5 79.46(15) . 3_767 ?
O8 V3 O5 76.14(14) . 3_767 ?
O4 V3 O5 75.42(14) 3_767 3_767 ?
O11 V3 V1 90.53(16) . 3_767 ?
O10 V3 V1 130.96(13) . 3_767 ?
O12 V3 V1 128.30(13) . 3_767 ?
O8 V3 V1 41.33(11) . 3_767 ?
O4 V3 V1 39.00(11) 3_767 3_767 ?
O5 V3 V1 84.40(10) 3_767 3_767 ?
O11 V3 V4 135.90(16) . . ?
O10 V3 V4 83.12(12) . . ?
O12 V3 V4 33.10(12) . . ?
O8 V3 V4 123.15(11) . . ?
O4 V3 V4 86.92(11) 3_767 . ?
O5 V3 V4 47.02(9) 3_767 . ?
V1 V3 V4 118.44(4) 3_767 . ?
O11 V3 V5 135.93(15) . . ?
O10 V3 V5 32.97(12) . . ?
O12 V3 V5 84.02(12) . . ?
O8 V3 V5 85.86(11) . . ?
O4 V3 V5 123.82(11) 3_767 . ?
O5 V3 V5 48.49(9) 3_767 . ?
V1 V3 V5 119.28(4) 3_767 . ?
V4 V3 V5 59.27(3) . . ?
O14 V4 O13 105.2(2) . . ?
O14 V4 O12 101.60(19) . . ?
O13 V4 O12 93.38(17) . . ?
O14 V4 O1 101.07(18) . . ?
O13 V4 O1 91.69(17) . . ?
O12 V4 O1 154.55(17) . . ?
O14 V4 O6 97.22(18) . 3_767 ?
O13 V4 O6 157.51(17) . 3_767 ?
O12 V4 O6 83.81(16) . 3_767 ?
O1 V4 O6 82.04(15) . 3_767 ?
O14 V4 O5 171.63(18) . 3_767 ?
O13 V4 O5 83.09(16) . 3_767 ?
O12 V4 O5 78.74(15) . 3_767 ?
O1 V4 O5 77.15(14) . 3_767 ?
O6 V4 O5 74.46(14) 3_767 3_767 ?
O14 V4 V2 128.54(15) . 3_767 ?
O13 V4 V2 126.21(13) . 3_767 ?
O12 V4 V2 79.50(12) . 3_767 ?
O1 V4 V2 77.41(12) . 3_767 ?
O6 V4 V2 31.33(10) 3_767 3_767 ?
O5 V4 V2 43.14(9) 3_767 3_767 ?
O14 V4 V5 139.11(15) . . ?
O13 V4 V5 33.93(12) . . ?
O12 V4 V5 85.00(12) . . ?
O1 V4 V5 85.40(11) . . ?
O6 V4 V5 123.66(11) 3_767 . ?
O5 V4 V5 49.20(9) 3_767 . ?
V2 V4 V5 92.34(4) 3_767 . ?
O14 V4 V3 134.33(15) . . ?
O13 V4 V3 83.36(12) . . ?
O12 V4 V3 32.75(12) . . ?
O1 V4 V3 123.79(12) . . ?
O6 V4 V3 82.32(11) 3_767 . ?
O5 V4 V3 46.64(9) 3_767 . ?
V2 V4 V3 62.25(3) 3_767 . ?
V5 V4 V3 60.63(3) . . ?
O14 V4 V1 134.06(15) . . ?
O13 V4 V1 80.89(13) . . ?
O12 V4 V1 123.77(12) . . ?
O1 V4 V1 33.08(11) . . ?
O6 V4 V1 82.20(11) 3_767 . ?
O5 V4 V1 45.04(9) 3_767 . ?
V2 V4 V1 61.49(3) 3_767 . ?
V5 V4 V1 59.90(3) . . ?
V3 V4 V1 91.35(3) . . ?
O9 V5 O10 102.8(2) . . ?
O9 V5 O13 103.5(2) . . ?
O10 V5 O13 91.37(17) . . ?
O9 V5 O3 101.9(2) . . ?
O10 V5 O3 154.62(17) . . ?
O13 V5 O3 88.80(17) . . ?
O9 V5 O7 100.9(2) . . ?
O10 V5 O7 84.92(16) . . ?
O13 V5 O7 155.51(16) . . ?
O3 V5 O7 84.49(16) . . ?
O9 V5 O5 176.2(2) . 3_767 ?
O10 V5 O5 78.31(15) . 3_767 ?
O13 V5 O5 80.03(15) . 3_767 ?
O3 V5 O5 76.73(14) . 3_767 ?
O7 V5 O5 75.51(14) . 3_767 ?
O9 V5 V2 132.07(17) . . ?
O10 V5 V2 79.65(12) . . ?
O13 V5 V2 124.35(12) . . ?
O3 V5 V2 79.36(12) . . ?
O7 V5 V2 31.19(11) . . ?
O5 V5 V2 44.32(9) 3_767 . ?
O9 V5 V4 136.33(17) . . ?
O10 V5 V4 83.41(12) . . ?
O13 V5 V4 32.79(12) . . ?
O3 V5 V4 83.07(12) . . ?
O7 V5 V4 122.78(11) . . ?
O5 V5 V4 47.27(9) 3_767 . ?
V2 V5 V4 91.59(3) . . ?
O9 V5 V1 133.41(16) . . ?
O10 V5 V1 123.67(12) . . ?
O13 V5 V1 80.84(12) . . ?
O3 V5 V1 31.57(11) . . ?
O7 V5 V1 81.16(11) . . ?
O5 V5 V1 45.36(9) 3_767 . ?
V2 V5 V1 61.23(3) . . ?
V4 V5 V1 60.71(3) . . ?
O9 V5 V3 135.05(16) . . ?
O10 V5 V3 32.36(12) . . ?
O13 V5 V3 82.07(12) . . ?
O3 V5 V3 122.97(12) . . ?
O7 V5 V3 81.93(11) . . ?
O5 V5 V3 46.24(9) 3_767 . ?
V2 V5 V3 61.53(3) . . ?
V4 V5 V3 60.10(3) . . ?
V1 V5 V3 91.51(3) . . ?
O39 V6 O18 105.0(2) . . ?
O39 V6 O22 99.06(18) . . ?
O18 V6 O22 100.49(17) . . ?
O39 V6 O30 98.95(18) . 3_666 ?
O18 V6 O30 99.07(17) . 3_666 ?
O22 V6 O30 148.87(16) . 3_666 ?
O39 V6 O25 163.64(17) . . ?
O18 V6 O25 91.33(17) . . ?
O22 V6 O25 78.24(15) . . ?
O30 V6 O25 77.32(14) 3_666 . ?
O39 V6 O28 89.59(17) . 3_666 ?
O18 V6 O28 165.37(17) . 3_666 ?
O22 V6 O28 77.69(14) . 3_666 ?
O30 V6 O28 77.28(14) 3_666 3_666 ?
O25 V6 O28 74.06(13) . 3_666 ?
O26 V7 O19 105.08(19) . . ?
O26 V7 O24 98.58(17) . . ?
O19 V7 O24 100.63(17) . . ?
O26 V7 O30 98.99(17) . 3_666 ?
O19 V7 O30 100.68(17) . 3_666 ?
O24 V7 O30 147.68(16) . 3_666 ?
O26 V7 O25 163.23(16) . . ?
O19 V7 O25 91.69(16) . . ?
O24 V7 O25 77.73(14) . . ?
O30 V7 O25 77.63(15) 3_666 . ?
O26 V7 O29 89.11(16) . 3_666 ?
O19 V7 O29 165.80(16) . 3_666 ?
O24 V7 O29 76.48(14) . 3_666 ?
O30 V7 O29 76.90(15) 3_666 3_666 ?
O25 V7 O29 74.12(13) . 3_666 ?
O27 V8 O20 104.43(19) . . ?
O27 V8 O23 99.73(18) . . ?
O20 V8 O23 99.50(17) . . ?
O27 V8 O24 98.26(18) . . ?
O20 V8 O24 99.80(17) . . ?
O23 V8 O24 149.32(16) . . ?
O27 V8 O25 164.49(17) . . ?
O20 V8 O25 91.04(17) . . ?
O23 V8 O25 78.42(15) . . ?
O24 V8 O25 77.62(14) . . ?
O27 V8 O28 90.33(17) . . ?
O20 V8 O28 165.25(17) . . ?
O23 V8 O28 77.60(14) . . ?
O24 V8 O28 77.66(14) . . ?
O25 V8 O28 74.21(13) . . ?
O33 V9 O21 104.40(19) . . ?
O33 V9 O23 100.04(19) . . ?
O21 V9 O23 99.19(18) . . ?
O33 V9 O22 99.77(18) . . ?
O21 V9 O22 99.71(18) . . ?
O23 V9 O22 148.14(15) . . ?
O33 V9 O29 90.68(17) . . ?
O21 V9 O29 164.92(17) . . ?
O23 V9 O29 77.88(15) . . ?
O22 V9 O29 77.19(15) . . ?
O33 V9 O25 164.96(17) . . ?
O21 V9 O25 90.64(16) . . ?
O23 V9 O25 77.15(14) . . ?
O22 V9 O25 77.23(14) . . ?
O29 V9 O25 74.28(13) . . ?
O31 V10 O43 104.8(2) . . ?
O31 V10 O22 100.72(17) . . ?
O43 V10 O22 99.46(18) . . ?
O31 V10 O24 99.85(17) . 3_666 ?
O43 V10 O24 97.61(18) . 3_666 ?
O22 V10 O24 148.83(15) . 3_666 ?
O31 V10 O29 92.00(17) . . ?
O43 V10 O29 163.18(17) . . ?
O22 V10 O29 77.82(15) . . ?
O24 V10 O29 78.31(15) 3_666 . ?
O31 V10 O28 165.29(18) . 3_666 ?
O43 V10 O28 89.88(17) . 3_666 ?
O22 V10 O28 77.38(14) . 3_666 ?
O24 V10 O28 76.78(14) 3_666 3_666 ?
O29 V10 O28 73.32(14) . 3_666 ?
O28 V11 O28 180.0 3_666 . ?
O28 V11 O29 90.12(16) 3_666 3_666 ?
O28 V11 O29 89.88(16) . 3_666 ?
O28 V11 O29 89.88(16) 3_666 . ?
O28 V11 O29 90.12(16) . . ?
O29 V11 O29 180.00(14) 3_666 . ?
O28 V11 O25 90.15(15) 3_666 . ?
O28 V11 O25 89.85(15) . . ?
O29 V11 O25 89.92(15) 3_666 . ?
O29 V11 O25 90.08(15) . . ?
O28 V11 O25 89.85(15) 3_666 3_666 ?
O28 V11 O25 90.15(15) . 3_666 ?
O29 V11 O25 90.08(15) 3_666 3_666 ?
O29 V11 O25 89.92(15) . 3_666 ?
O25 V11 O25 180.0 . 3_666 ?
O44 V12 O32 104.8(2) . . ?
O44 V12 O23 99.00(18) . . ?
O32 V12 O23 100.07(18) . . ?
O44 V12 O30 99.16(18) . . ?
O32 V12 O30 98.54(17) . . ?
O23 V12 O30 149.63(16) . . ?
O44 V12 O28 90.75(17) . . ?
O32 V12 O28 164.39(18) . . ?
O23 V12 O28 77.91(14) . . ?
O30 V12 O28 77.71(14) . . ?
O44 V12 O29 164.56(17) . . ?
O32 V12 O29 90.61(17) . . ?
O23 V12 O29 77.93(15) . . ?
O30 V12 O29 78.08(15) . . ?
O28 V12 O29 73.81(13) . . ?
V1 O1 V4 112.96(18) . . ?
V1 O1 La1 101.56(16) . . ?
V4 O1 La1 144.24(19) . . ?
V1 O2 La1 102.60(18) . . ?
V1 O3 V5 114.48(19) . . ?
V2 O4 V1 106.96(18) . . ?
V2 O4 V3 107.36(17) . 3_767 ?
V1 O4 V3 101.05(16) . 3_767 ?
V2 O5 V2 101.76(15) . 3_767 ?
V2 O5 V1 94.49(14) . 3_767 ?
V2 O5 V1 92.16(14) 3_767 3_767 ?
V2 O5 V3 93.98(14) . 3_767 ?
V2 O5 V3 91.72(13) 3_767 3_767 ?
V1 O5 V3 169.77(19) 3_767 3_767 ?
V2 O5 V4 88.61(13) . 3_767 ?
V2 O5 V4 169.57(19) 3_767 3_767 ?
V1 O5 V4 88.14(13) 3_767 3_767 ?
V3 O5 V4 86.34(13) 3_767 3_767 ?
V2 O5 V5 172.13(19) . 3_767 ?
V2 O5 V5 86.10(13) 3_767 3_767 ?
V1 O5 V5 85.56(12) 3_767 3_767 ?
V3 O5 V5 85.27(12) 3_767 3_767 ?
V4 O5 V5 83.53(12) 3_767 3_767 ?
V2 O6 V4 108.34(18) . 3_767 ?
V2 O7 V5 111.67(19) . . ?
V2 O8 V3 109.14(17) . . ?
V2 O8 V1 106.05(17) . 3_767 ?
V3 O8 V1 98.76(16) . 3_767 ?
V3 O10 V5 114.67(19) . . ?
V3 O12 V4 114.2(2) . . ?
V4 O13 V5 113.3(2) . . ?
La1 O15 H15A 129(6) . . ?
La1 O15 H15B 116(6) . . ?
H15A O15 H15B 99(8) . . ?
La1 O16 H16A 122(7) . . ?
La1 O16 H16B 130(6) . . ?
H16A O16 H16B 82(8) . . ?
La1 O17 H17A 143(5) . . ?
La1 O17 H17B 114(5) . . ?
H17A O17 H17B 102(7) . . ?
V6 O18 La1 132.2(2) . . ?
V7 O19 La1 130.94(19) . . ?
V8 O20 La1 131.8(2) . . ?
V9 O21 La1 132.78(19) . . ?
V9 O22 V10 108.41(18) . . ?
V9 O22 V6 109.63(18) . . ?
V10 O22 V6 110.07(17) . . ?
V12 O23 V9 108.69(17) . . ?
V12 O23 V8 109.14(18) . . ?
V9 O23 V8 109.71(19) . . ?
V7 O24 V8 108.40(17) . . ?
V7 O24 V10 109.45(18) . 3_666 ?
V8 O24 V10 110.21(18) . 3_666 ?
V11 O25 V7 98.76(14) . . ?
V11 O25 V8 97.42(15) . . ?
V7 O25 V8 89.32(13) . . ?
V11 O25 V6 97.46(15) . . ?
V7 O25 V6 89.46(14) . . ?
V8 O25 V6 165.09(18) . . ?
V11 O25 V9 96.74(15) . . ?
V7 O25 V9 164.50(18) . . ?
V8 O25 V9 88.59(13) . . ?
V6 O25 V9 88.63(13) . . ?
V7 O26 La2 136.0(2) . 3_666 ?
V8 O27 La3 135.8(2) . 3_666 ?
V11 O28 V12 98.53(15) . . ?
V11 O28 V8 98.52(16) . . ?
V12 O28 V8 88.71(13) . . ?
V11 O28 V6 98.33(15) . 3_666 ?
V12 O28 V6 89.16(13) . 3_666 ?
V8 O28 V6 163.15(19) . 3_666 ?
V11 O28 V10 97.79(16) . 3_666 ?
V12 O28 V10 163.67(19) . 3_666 ?
V8 O28 V10 89.02(13) . 3_666 ?
V6 O28 V10 88.34(13) 3_666 3_666 ?
V11 O29 V10 99.01(16) . . ?
V11 O29 V12 97.54(15) . . ?
V10 O29 V12 163.45(18) . . ?
V11 O29 V9 98.89(16) . . ?
V10 O29 V9 89.17(14) . . ?
V12 O29 V9 88.58(13) . . ?
V11 O29 V7 97.20(15) . 3_666 ?
V10 O29 V7 88.87(13) . 3_666 ?
V12 O29 V7 88.76(14) . 3_666 ?
V9 O29 V7 163.89(18) . 3_666 ?
V7 O30 V6 108.65(18) 3_666 3_666 ?
V7 O30 V12 110.00(18) 3_666 . ?
V6 O30 V12 109.16(17) 3_666 . ?
V10 O31 La2 133.3(2) . . ?
V12 O32 La2 134.9(2) . . ?
V9 O33 La2 134.7(2) . . ?
La2 O34 H34A 114(6) . . ?
La2 O34 H34B 132(6) . . ?
H34A O34 H34B 113(8) . . ?
La2 O35 H35A 112(5) . . ?
La2 O35 H35B 126(5) . . ?
H35A O35 H35B 105(7) . . ?
La2 O36 H36A 127(6) . . ?
La2 O36 H36B 138(6) . . ?
H36A O36 H36B 95(8) . . ?
La2 O37 H37A 117(9) . . ?
La2 O37 H37B 126(7) . . ?
H37A O37 H37B 117(10) . . ?
La2 O38 H38A 129(7) . . ?
La2 O38 H38B 125(7) . . ?
H38A O38 H38B 103(9) . . ?
V6 O39 La3 137.2(2) . . ?
La3 O40 H40A 117(7) . . ?
La3 O40 H40B 109(7) . . ?
H40A O40 H40B 134(10) . . ?
La3 O41A H41A 117(7) . . ?
La3 O41A H41B 107(7) . . ?
H41A O41A H41B 124(10) . . ?
La3 O42 H42A 124(6) . . ?
La3 O42 H42B 131(6) . . ?
H42A O42 H42B 104(8) . . ?
V10 O43 La3 136.2(2) . . ?
V12 O44 La3 135.2(2) . 3_666 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 V1 O1 V4 173.8(2) . . . . ?
O3 V1 O1 V4 69.2(2) . . . . ?
O4 V1 O1 V4 -40.0(5) . . . . ?
O8 V1 O1 V4 -88.3(2) 3_767 . . . ?
O5 V1 O1 V4 -12.39(18) 3_767 . . . ?
V3 V1 O1 V4 -89.06(19) 3_767 . . . ?
V5 V1 O1 V4 36.78(16) . . . . ?
La1 V1 O1 V4 170.5(3) . . . . ?
O2 V1 O1 La1 3.34(18) . . . . ?
O3 V1 O1 La1 -101.31(16) . . . . ?
O4 V1 O1 La1 149.6(3) . . . . ?
O8 V1 O1 La1 101.25(15) 3_767 . . . ?
O5 V1 O1 La1 177.15(16) 3_767 . . . ?
V3 V1 O1 La1 100.48(13) 3_767 . . . ?
V5 V1 O1 La1 -133.68(11) . . . . ?
V4 V1 O1 La1 -170.5(3) . . . . ?
O14 V4 O1 V1 -176.2(2) . . . . ?
O13 V4 O1 V1 -70.4(2) . . . . ?
O12 V4 O1 V1 31.1(5) . . . . ?
O6 V4 O1 V1 87.9(2) 3_767 . . . ?
O5 V4 O1 V1 12.13(17) 3_767 . . . ?
V2 V4 O1 V1 56.41(16) 3_767 . . . ?
V5 V4 O1 V1 -37.02(17) . . . . ?
V3 V4 O1 V1 12.8(2) . . . . ?
O14 V4 O1 La1 -12.4(4) . . . . ?
O13 V4 O1 La1 93.5(3) . . . . ?
O12 V4 O1 La1 -165.0(3) . . . . ?
O6 V4 O1 La1 -108.2(3) 3_767 . . . ?
O5 V4 O1 La1 176.0(3) 3_767 . . . ?
V2 V4 O1 La1 -139.7(3) 3_767 . . . ?
V5 V4 O1 La1 126.9(3) . . . . ?
V3 V4 O1 La1 176.6(2) . . . . ?
V1 V4 O1 La1 163.9(5) . . . . ?
O3 V1 O2 La1 94.61(18) . . . . ?
O1 V1 O2 La1 -3.17(17) . . . . ?
O4 V1 O2 La1 -169.15(14) . . . . ?
O8 V1 O2 La1 -91.15(16) 3_767 . . . ?
V3 V1 O2 La1 -130.76(11) 3_767 . . . ?
V5 V1 O2 La1 87.0(2) . . . . ?
V4 V1 O2 La1 1.3(2) . . . . ?
O2 V1 O3 V5 -170.8(2) . . . . ?
O1 V1 O3 V5 -72.9(2) . . . . ?
O4 V1 O3 V5 83.6(2) . . . . ?
O8 V1 O3 V5 24.1(6) 3_767 . . . ?
O5 V1 O3 V5 5.9(2) 3_767 . . . ?
V3 V1 O3 V5 83.5(2) 3_767 . . . ?
V4 V1 O3 V5 -41.22(18) . . . . ?
La1 V1 O3 V5 -119.60(18) . . . . ?
O9 V5 O3 V1 177.9(2) . . . . ?
O10 V5 O3 V1 -16.3(5) . . . . ?
O13 V5 O3 V1 74.3(2) . . . . ?
O7 V5 O3 V1 -82.1(2) . . . . ?
O5 V5 O3 V1 -5.70(19) 3_767 . . . ?
V2 V5 O3 V1 -50.98(18) . . . . ?
V4 V5 O3 V1 41.95(18) . . . . ?
V3 V5 O3 V1 -5.4(3) . . . . ?
O7 V2 O6 V4 179.37(17) . . . 3_767 ?
O8 V2 O6 V4 -81.23(19) . . . 3_767 ?
O4 V2 O6 V4 80.41(19) . . . 3_767 ?
O5 V2 O6 V4 -0.04(18) . . . 3_767 ?
O5 V2 O6 V4 4.8(8) 3_767 . . 3_767 ?
V5 V2 O6 V4 179.00(7) . . . 3_767 ?
O6 V2 O7 V5 -179.64(19) . . . . ?
O8 V2 O7 V5 79.1(2) . . . . ?
O4 V2 O7 V5 -80.1(2) . . . . ?
O5 V2 O7 V5 -1.9(8) . . . . ?
O5 V2 O7 V5 -0.89(19) 3_767 . . . ?
V4 V2 O7 V5 -178.89(8) 3_767 . . . ?
O11 V3 O10 V5 176.2(2) . . . . ?
O12 V3 O10 V5 71.7(2) . . . . ?
O8 V3 O10 V5 -82.9(2) . . . . ?
O4 V3 O10 V5 -26.6(5) 3_767 . . . ?
O5 V3 O10 V5 -6.9(2) 3_767 . . . ?
V1 V3 O10 V5 -81.5(2) 3_767 . . . ?
V4 V3 O10 V5 40.55(18) . . . . ?
O9 V5 O10 V3 -177.0(2) . . . . ?
O13 V5 O10 V3 -72.8(2) . . . . ?
O3 V5 O10 V3 17.3(5) . . . . ?
O7 V5 O10 V3 82.9(2) . . . . ?
O5 V5 O10 V3 6.71(19) 3_767 . . . ?
V2 V5 O10 V3 51.89(18) . . . . ?
V4 V5 O10 V3 -40.94(18) . . . . ?
V1 V5 O10 V3 7.1(3) . . . . ?
O11 V3 O12 V4 -174.5(2) . . . . ?
O10 V3 O12 V4 -70.0(2) . . . . ?
O8 V3 O12 V4 28.7(5) . . . . ?
O4 V3 O12 V4 85.4(2) 3_767 . . . ?
O5 V3 O12 V4 10.12(19) 3_767 . . . ?
V1 V3 O12 V4 84.2(2) 3_767 . . . ?
V5 V3 O12 V4 -38.71(18) . . . . ?
O14 V4 O12 V3 178.5(2) . . . . ?
O13 V4 O12 V3 72.2(2) . . . . ?
O1 V4 O12 V3 -28.9(5) . . . . ?
O6 V4 O12 V3 -85.4(2) 3_767 . . . ?
O5 V4 O12 V3 -10.08(19) 3_767 . . . ?
V2 V4 O12 V3 -54.04(18) 3_767 . . . ?
V5 V4 O12 V3 39.27(18) . . . . ?
V1 V4 O12 V3 -9.1(3) . . . . ?
O14 V4 O13 V5 -178.9(2) . . . . ?
O12 V4 O13 V5 -75.9(2) . . . . ?
O1 V4 O13 V5 79.2(2) . . . . ?
O6 V4 O13 V5 6.1(5) 3_767 . . . ?
O5 V4 O13 V5 2.35(19) 3_767 . . . ?
V2 V4 O13 V5 3.6(3) 3_767 . . . ?
V3 V4 O13 V5 -44.64(17) . . . . ?
V1 V4 O13 V5 47.81(17) . . . . ?
O9 V5 O13 V4 179.0(2) . . . . ?
O10 V5 O13 V4 75.6(2) . . . . ?
O3 V5 O13 V4 -79.0(2) . . . . ?
O7 V5 O13 V4 -5.2(5) . . . . ?
O5 V5 O13 V4 -2.30(18) 3_767 . . . ?
V2 V5 O13 V4 -2.8(3) . . . . ?
V1 V5 O13 V4 -48.33(17) . . . . ?
V3 V5 O13 V4 44.50(17) . . . . ?
O39 V6 O18 La1 177.3(2) . . . . ?
O22 V6 O18 La1 74.8(3) . . . . ?
O30 V6 O18 La1 -80.8(3) 3_666 . . . ?
O25 V6 O18 La1 -3.4(3) . . . . ?
O28 V6 O18 La1 -6.5(8) 3_666 . . . ?
O26 V7 O19 La1 179.1(2) . . . . ?
O24 V7 O19 La1 -78.9(3) . . . . ?
O30 V7 O19 La1 76.7(3) 3_666 . . . ?
O25 V7 O19 La1 -1.1(3) . . . . ?
O29 V7 O19 La1 -2.1(9) 3_666 . . . ?
O27 V8 O20 La1 -179.1(2) . . . . ?
O23 V8 O20 La1 -76.4(3) . . . . ?
O24 V8 O20 La1 79.6(3) . . . . ?
O25 V8 O20 La1 2.0(2) . . . . ?
O28 V8 O20 La1 0.9(8) . . . . ?
O33 V9 O21 La1 -178.6(3) . . . . ?
O23 V9 O21 La1 78.5(3) . . . . ?
O22 V9 O21 La1 -75.8(3) . . . . ?
O29 V9 O21 La1 1.0(9) . . . . ?
O25 V9 O21 La1 1.4(3) . . . . ?
O19 V7 O26 La2 -179.0(3) . . . 3_666 ?
O24 V7 O26 La2 77.5(3) . . . 3_666 ?
O30 V7 O26 La2 -75.3(3) 3_666 . . 3_666 ?
O25 V7 O26 La2 1.6(8) . . . 3_666 ?
O29 V7 O26 La2 1.3(3) 3_666 . . 3_666 ?
O20 V8 O27 La3 179.5(3) . . . 3_666 ?
O23 V8 O27 La3 77.0(3) . . . 3_666 ?
O24 V8 O27 La3 -78.0(3) . . . 3_666 ?
O25 V8 O27 La3 -4.7(8) . . . 3_666 ?
O28 V8 O27 La3 -0.5(3) . . . 3_666 ?
O29 V11 O28 V12 -179.77(15) 3_666 . . . ?
O29 V11 O28 V12 0.23(15) . . . . ?
O25 V11 O28 V12 90.31(15) . . . . ?
O25 V11 O28 V12 -89.69(15) 3_666 . . . ?
O29 V11 O28 V8 90.26(15) 3_666 . . . ?
O29 V11 O28 V8 -89.74(15) . . . . ?
O25 V11 O28 V8 0.34(15) . . . . ?
O25 V11 O28 V8 -179.66(15) 3_666 . . . ?
O29 V11 O28 V6 -89.37(15) 3_666 . . 3_666 ?
O29 V11 O28 V6 90.63(15) . . . 3_666 ?
O25 V11 O28 V6 -179.29(15) . . . 3_666 ?
O25 V11 O28 V6 0.71(15) 3_666 . . 3_666 ?
O29 V11 O28 V10 0.08(15) 3_666 . . 3_666 ?
O29 V11 O28 V10 -179.92(15) . . . 3_666 ?
O25 V11 O28 V10 -89.84(15) . . . 3_666 ?
O25 V11 O28 V10 90.16(15) 3_666 . . 3_666 ?
O43 V10 O31 La2 179.5(2) . . . . ?
O22 V10 O31 La2 -77.6(3) . . . . ?
O24 V10 O31 La2 78.9(3) 3_666 . . . ?
O29 V10 O31 La2 0.4(3) . . . . ?
O28 V10 O31 La2 3.5(8) 3_666 . . . ?
O44 V12 O32 La2 179.2(3) . . . . ?
O23 V12 O32 La2 77.0(3) . . . . ?
O30 V12 O32 La2 -78.9(3) . . . . ?
O28 V12 O32 La2 -4.1(8) . . . . ?
O29 V12 O32 La2 -0.8(3) . . . . ?
O21 V9 O33 La2 -179.2(3) . . . . ?
O23 V9 O33 La2 -76.9(3) . . . . ?
O22 V9 O33 La2 78.1(3) . . . . ?
O29 V9 O33 La2 0.9(3) . . . . ?
O25 V9 O33 La2 1.0(9) . . . . ?
O18 V6 O39 La3 180.0(3) . . . . ?
O22 V6 O39 La3 -76.5(3) . . . . ?
O30 V6 O39 La3 78.0(3) 3_666 . . . ?
O25 V6 O39 La3 2.6(9) . . . . ?
O28 V6 O39 La3 1.0(3) 3_666 . . . ?
O31 V10 O43 La3 179.0(3) . . . . ?
O22 V10 O43 La3 75.2(3) . . . . ?
O24 V10 O43 La3 -78.7(3) 3_666 . . . ?
O29 V10 O43 La3 -4.0(8) . . . . ?
O28 V10 O43 La3 -2.0(3) 3_666 . . . ?
O32 V12 O44 La3 178.4(3) . . . 3_666 ?
O23 V12 O44 La3 -78.5(3) . . . 3_666 ?
O30 V12 O44 La3 77.0(3) . . . 3_666 ?
O28 V12 O44 La3 -0.7(3) . . . 3_666 ?
O29 V12 O44 La3 -1.3(9) . . . 3_666 ?

_refine_diff_density_max         2.284
_refine_diff_density_min         -1.059
_refine_diff_density_rms         0.162



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_twin
_database_code_depnum_ccdc_archive 'CCDC 2341649'
loop_
_audit_author_name
_audit_author_address
'Robert Gyepes'
;Charles University
Czech Republic
;
_audit_update_record             
;
2024-03-20 deposited with the CCDC.	2024-12-12 downloaded from the CCDC.
;
_audit_creation_date             2024-02-02
_audit_creation_method           
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_shelx_SHELXL_version_number     2019/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'H28 La2 O42 V10, 8(O)'
_chemical_formula_sum            'H28 La2 O50 V10'
_chemical_formula_weight         1615.44
_chemical_melting_point          ?
_chemical_oxdiff_formula         'La2 H62 O54 V10'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   10.4779(2)
_cell_length_b                   11.2361(2)
_cell_length_c                   11.6788(3)
_cell_angle_alpha                114.085(2)
_cell_angle_beta                 99.949(2)
_cell_angle_gamma                99.5610(19)
_cell_volume                     1192.82(5)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    20155
_cell_measurement_temperature    160.00(10)
_cell_measurement_theta_max      32.6140
_cell_measurement_theta_min      5.6590
_shelx_estimated_absorpt_T_max   0.853
_shelx_estimated_absorpt_T_min   0.563
_exptl_absorpt_coefficient_mu    3.726
_exptl_absorpt_correction_T_max  0.871
_exptl_absorpt_correction_T_min  0.662
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.43.105a (Rigaku Oxford Diffraction, 2024)
Analytical numeric absorption correction using a multifaceted crystal
model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    2.249
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             772
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
-1 0 0 0.0183
5 -1 0 0.0182
-1 -5 5 0.0498
-2 1 5 0.0663
1 4 -5 0.0459
2 -1 -5 0.0663

_exptl_crystal_size_max          0.174
_exptl_crystal_size_mid          0.093
_exptl_crystal_size_min          0.044
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
-0.9995 -0.0016 0.0042 0.0644 -0.0284 0.0104
4.9961 -0.9914 -0.0191 -0.3180 0.1295 0.0182
-0.9876 -4.9914 4.9978 -0.0888 -0.3214 0.1734
-1.9793 1.0043 4.9904 -0.0481 -0.2748 -0.2386
0.9863 3.9918 -4.9958 0.0927 0.3089 -0.1030
1.9793 -1.0043 -4.9904 0.0481 0.2748 0.2386

_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  ?
_diffrn_reflns_av_unetI/netI     0.0219
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            15508
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.846
_diffrn_reflns_theta_min         2.439
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      160.00(10)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 5.8140
_diffrn_detector_type            'Pilatus 200K'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -11.00  90.00   0.50    4.00    --   14.46  57.00 -60.00  202
  2  ω    -61.00  40.00   0.50    4.00    --   14.46 -57.00   0.00  202
  3  ω    -91.00  10.00   0.50    4.00    --  -15.40 -57.00 120.00  202
  4  ω    -40.00  66.00   0.50    4.00    --  -15.40  38.00 -90.00  212
  5  ω    -90.00  10.00   0.50    4.00    --  -15.40 -60.00 -23.15  200
  6  ω    -91.00  10.00   0.50    4.00    --  -15.40 -57.00-120.00  202
  7  ω    -90.00  10.00   0.50    4.00    --  -15.40 -59.00 176.48  200
  8  ω    -90.00  10.00   0.50    4.00    --  -15.40 -60.00  75.91  200
  9  ω    -61.00  -7.00   0.50    4.00    --   14.46 -57.00 -90.00  108
 10  ω    -40.00  60.00   0.50    4.00    --  -15.40  57.00  90.00  200
 11  ω    -40.00  60.00   0.50    4.00    --  -15.40  57.00 150.00  200
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, Pilatus 200K'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0645719000
_diffrn_orient_matrix_UB_12      -0.0039439000
_diffrn_orient_matrix_UB_13      -0.0344623000
_diffrn_orient_matrix_UB_21      0.0281988000
_diffrn_orient_matrix_UB_22      0.0123728000
_diffrn_orient_matrix_UB_23      -0.0463777000
_diffrn_orient_matrix_UB_31      -0.0104968000
_diffrn_orient_matrix_UB_32      -0.0704858000
_diffrn_orient_matrix_UB_33      -0.0377806000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                13789
_reflns_number_total             15508
_reflns_special_details          
;
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.43.105a (Rigaku OD, 2024)'
_computing_data_collection       
'CrysAlisPro system (CCD 41.123a 64-bit (release 20-01-2022))'
_computing_data_reduction        'CrysAlisPro 1.171.43.105a (Rigaku OD, 2024)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/3 (Sheldrick, 2015)'
_computing_structure_solution    ?
_refine_diff_density_max         3.222
_refine_diff_density_min         -1.559
_refine_diff_density_rms         0.209
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     290
_refine_ls_number_reflns         15508
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0530
_refine_ls_R_factor_gt           0.0462
_refine_ls_restrained_S_all      1.029
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0686P)²+6.8098P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1232
_refine_ls_wR_factor_ref         0.1302
_refine_special_details          
;
 Refined as a 2-component twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.6294(11)
 0.3706(11)
2. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
3.a Free rotating group:
 O4W(H4WA,H4WB)
3.b Rotating group:
 O7W(H7WA,H7WB), O6W(H6WA,H6WB), O1W(H1WA,H1WB), O5W(H5WA,H5WB), O3W(H3WA,
 H3WB), O2W(H2WA,H2WB)
;
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.86092(2) 0.52196(3) 0.71860(2) 0.01428(8) Uani 1 1 d . . . . .
V002 V 0.92176(7) -0.25180(8) 0.30466(7) 0.01226(15) Uani 1 1 d . . . . .
V003 V 0.89247(7) -0.04457(8) 0.57322(7) 0.01168(15) Uani 1 1 d . . . . .
V004 V 0.66870(7) -0.14116(8) 0.32237(8) 0.01525(16) Uani 1 1 d . . . . .
V005 V 0.86558(8) -0.05975(8) 0.18433(7) 0.01529(16) Uani 1 1 d . . . . .
V006 V 0.84693(7) 0.15152(8) 0.44821(7) 0.01313(15) Uani 1 1 d . . . . .
O7 O 0.9517(3) -0.2047(3) 0.4938(3) 0.0124(6) Uani 1 1 d . . . . .
O5 O 0.8887(3) 0.1366(3) 0.6158(3) 0.0126(6) Uani 1 1 d . . . . .
O12 O 0.8992(3) -0.0434(3) 0.3940(3) 0.0120(6) Uani 1 1 d . . . . .
O6 O 0.9328(3) -0.0279(3) 0.7265(3) 0.0158(6) Uani 1 1 d . . . . .
O8 O 0.9144(3) -0.2186(3) 0.1653(3) 0.0146(6) Uani 1 1 d . . . . .
O13 O 0.7263(3) -0.1177(3) 0.5091(3) 0.0153(6) Uani 1 1 d . . . . .
O1 O 0.9581(3) -0.3974(3) 0.2564(3) 0.0151(6) Uani 1 1 d . . . . .
O11 O 0.8279(3) 0.3047(3) 0.5091(3) 0.0167(6) Uani 1 1 d . . . . .
O2 O 0.7421(3) -0.2921(3) 0.2838(3) 0.0148(6) Uani 1 1 d . . . . .
O10 O 0.8537(3) 0.1166(3) 0.2849(3) 0.0156(6) Uani 1 1 d . . . . .
O16 O 0.6937(3) -0.1326(3) 0.1750(3) 0.0159(6) Uani 1 1 d . . . . .
O4 O 0.6798(3) 0.0430(3) 0.4034(3) 0.0158(6) Uani 1 1 d . . . . .
O7W O 0.8619(5) 0.5683(4) 0.5204(4) 0.0323(9) Uani 1 1 d . . . . .
H7WA H 0.932991 0.640880 0.538735 0.048 Uiso 1 1 d R U . . .
H7WB H 0.787710 0.597247 0.496972 0.048 Uiso 1 1 d R U . . .
O6W O 1.0995(4) 0.6407(4) 0.7291(4) 0.0284(8) Uani 1 1 d . . . . .
H6WA H 1.158616 0.659753 0.804476 0.043 Uiso 1 1 d R U . . .
H6WB H 1.102689 0.723369 0.733248 0.043 Uiso 1 1 d R U . . .
O1W O 0.7657(4) 0.3216(4) 0.7591(4) 0.0222(7) Uani 1 1 d . . . . .
H1WA H 0.789141 0.250529 0.710250 0.033 Uiso 1 1 d R U . . .
H1WB H 0.678006 0.298303 0.732080 0.033 Uiso 1 1 d R U . . .
O5W O 0.9867(4) 0.6086(4) 0.9589(4) 0.0275(8) Uani 1 1 d . . . . .
H5WA H 0.968658 0.687371 1.012135 0.041 Uiso 1 1 d R U . . .
H5WB H 1.078547 0.635147 0.972665 0.041 Uiso 1 1 d R U . . .
O9 O 0.8586(4) -0.0642(4) 0.0451(3) 0.0235(7) Uani 1 1 d . . . . .
O3 O 0.5112(3) -0.2109(4) 0.2855(4) 0.0228(7) Uani 1 1 d . . . . .
O3W O 0.7076(4) 0.5961(5) 0.8595(4) 0.0302(9) Uani 1 1 d . . . . .
H3WA H 0.686400 0.567138 0.916848 0.045 Uiso 1 1 d R U . . .
H3WB H 0.661218 0.657800 0.864295 0.045 Uiso 1 1 d R U . . .
O4W O 0.8588(5) 0.7652(4) 0.7895(4) 0.0342(10) Uani 1 1 d G . . . .
H4WA H 0.885317 0.831873 0.771924 0.051 Uiso 1 1 d G U . . .
H4WB H 0.870691 0.802971 0.873366 0.051 Uiso 1 1 d G U . . .
O2W O 0.6227(4) 0.4402(5) 0.5775(4) 0.0375(11) Uani 1 1 d . . . . .
H2WA H 0.558020 0.483408 0.587396 0.056 Uiso 1 1 d R U . . .
H2WB H 0.584245 0.361537 0.506497 0.056 Uiso 1 1 d R U . . .
O19 O 0.6343(4) 0.5123(4) 1.0302(4) 0.0266(8) Uani 1 1 d . . . . .
O17 O 0.4828(5) 0.1715(6) 0.3796(6) 0.0445(12) Uani 1 1 d . . . . .
O18 O 0.3924(5) 0.4742(7) 0.6454(6) 0.0530(14) Uani 1 1 d . . . . .
O20 O 0.5249(7) 0.7282(9) 0.8016(8) 0.075(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 O1 2.581(3) 2_756 ?
La1 O11 2.572(3) . ?
La1 O7W 2.572(4) . ?
La1 O6W 2.588(4) . ?
La1 O1W 2.564(4) . ?
La1 O5W 2.574(4) . ?
La1 O3W 2.494(4) . ?
La1 O4W 2.517(4) . ?
La1 O2W 2.524(4) . ?
V002 V004 3.1135(11) . ?
V002 V005 3.0966(11) . ?
V002 V006 3.0815(10) 2_756 ?
V002 O7 2.002(3) . ?
V002 O5 2.003(3) 2_756 ?
V002 O12 2.214(3) . ?
V002 O8 1.805(3) . ?
V002 O1 1.633(3) . ?
V002 O2 1.810(3) . ?
V003 V004 3.0731(11) . ?
V003 V005 3.1052(11) 2_756 ?
V003 O7 1.921(3) . ?
V003 O5 1.898(3) . ?
V003 O12 2.111(3) . ?
V003 O12 2.139(3) 2_756 ?
V003 O6 1.690(3) . ?
V003 O13 1.685(3) . ?
V004 V005 3.0687(11) . ?
V004 V006 3.0870(11) . ?
V004 O12 2.326(3) . ?
V004 O13 2.052(3) . ?
V004 O2 1.898(3) . ?
V004 O16 1.822(3) . ?
V004 O4 1.864(4) . ?
V004 O3 1.604(3) . ?
V005 V006 3.0923(11) . ?
V005 O12 2.339(3) . ?
V005 O6 2.056(3) 2_756 ?
V005 O8 1.875(4) . ?
V005 O10 1.885(4) . ?
V005 O16 1.816(3) . ?
V005 O9 1.595(4) . ?
V006 O7 2.006(3) 2_756 ?
V006 O5 2.012(3) . ?
V006 O12 2.210(3) . ?
V006 O11 1.635(4) . ?
V006 O10 1.801(3) . ?
V006 O4 1.811(3) . ?
O7W H7WA 0.9310 . ?
O7W H7WB 0.9318 . ?
O6W H6WA 0.9042 . ?
O6W H6WB 0.9047 . ?
O1W H1WA 0.8747 . ?
O1W H1WB 0.8744 . ?
O5W H5WA 0.9238 . ?
O5W H5WB 0.9238 . ?
O3W H3WA 0.9000 . ?
O3W H3WB 0.8995 . ?
O4W H4WA 0.8697 . ?
O4W H4WB 0.8700 . ?
O2W H2WA 0.8938 . ?
O2W H2WB 0.8938 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O6W 65.07(12) 2_756 . ?
O11 La1 O1 68.37(10) . 2_756 ?
O11 La1 O6W 97.02(12) . . ?
O11 La1 O5W 134.19(12) . . ?
O7W La1 O1 109.09(14) . 2_756 ?
O7W La1 O11 67.78(13) . . ?
O7W La1 O6W 68.40(14) . . ?
O7W La1 O5W 142.39(14) . . ?
O1W La1 O1 69.61(11) . 2_756 ?
O1W La1 O11 72.53(12) . . ?
O1W La1 O7W 136.87(13) . . ?
O1W La1 O6W 134.04(13) . . ?
O1W La1 O5W 79.16(14) . . ?
O5W La1 O1 68.31(11) . 2_756 ?
O5W La1 O6W 77.65(14) . . ?
O3W La1 O1 128.26(13) . 2_756 ?
O3W La1 O11 131.09(13) . . ?
O3W La1 O7W 122.64(15) . . ?
O3W La1 O6W 131.84(14) . . ?
O3W La1 O1W 73.58(13) . . ?
O3W La1 O5W 70.11(14) . . ?
O3W La1 O4W 66.27(14) . . ?
O3W La1 O2W 70.87(15) . . ?
O4W La1 O1 135.24(14) . 2_756 ?
O4W La1 O11 139.82(13) . . ?
O4W La1 O7W 72.93(14) . . ?
O4W La1 O6W 75.60(15) . . ?
O4W La1 O1W 139.65(12) . . ?
O4W La1 O5W 83.60(15) . . ?
O4W La1 O2W 91.73(17) . . ?
O2W La1 O1 132.30(14) . 2_756 ?
O2W La1 O11 68.68(13) . . ?
O2W La1 O7W 71.93(16) . . ?
O2W La1 O6W 140.31(16) . . ?
O2W La1 O1W 78.61(16) . . ?
O2W La1 O5W 139.10(14) . . ?
V005 V002 V004 59.23(3) . . ?
V006 V002 V004 119.72(3) 2_756 . ?
V006 V002 V005 120.36(3) 2_756 . ?
O7 V002 V004 87.37(9) . . ?
O7 V002 V005 124.92(10) . . ?
O7 V002 V006 39.80(9) . 2_756 ?
O7 V002 O5 76.42(13) . 2_756 ?
O7 V002 O12 76.08(13) . . ?
O5 V002 V004 124.50(10) 2_756 . ?
O5 V002 V005 87.83(10) 2_756 . ?
O5 V002 V006 39.97(9) 2_756 2_756 ?
O5 V002 O12 76.32(12) 2_756 . ?
O12 V002 V004 48.21(8) . . ?
O12 V002 V005 48.86(8) . . ?
O12 V002 V006 84.77(8) . 2_756 ?
O8 V002 V004 84.27(11) . . ?
O8 V002 V005 33.42(11) . . ?
O8 V002 V006 129.95(11) . 2_756 ?
O8 V002 O7 156.06(15) . . ?
O8 V002 O5 89.98(14) . 2_756 ?
O8 V002 O12 81.66(14) . . ?
O8 V002 O2 95.51(15) . . ?
O1 V002 V004 138.46(12) . . ?
O1 V002 V005 136.47(12) . . ?
O1 V002 V006 86.89(12) . 2_756 ?
O1 V002 O7 98.02(15) . . ?
O1 V002 O5 96.61(15) . 2_756 ?
O1 V002 O12 171.61(15) . . ?
O1 V002 O8 103.10(16) . . ?
O1 V002 O2 104.78(16) . . ?
O2 V002 V004 33.78(11) . . ?
O2 V002 V005 84.10(11) . . ?
O2 V002 V006 129.61(11) . 2_756 ?
O2 V002 O7 89.80(14) . . ?
O2 V002 O5 156.02(14) . 2_756 ?
O2 V002 O12 81.40(14) . . ?
V004 V003 V005 175.44(3) . 2_756 ?
O7 V003 V004 89.98(10) . . ?
O7 V003 V005 89.03(10) . 2_756 ?
O7 V003 O12 79.68(13) . 2_756 ?
O7 V003 O12 80.29(13) . . ?
O5 V003 V004 89.54(10) . . ?
O5 V003 V005 89.45(10) . 2_756 ?
O5 V003 O7 154.67(14) . . ?
O5 V003 O12 80.31(13) . . ?
O5 V003 O12 80.35(13) . 2_756 ?
O12 V003 V004 126.63(9) 2_756 . ?
O12 V003 V004 49.12(8) . . ?
O12 V003 V005 126.33(9) . 2_756 ?
O12 V003 V005 48.81(8) 2_756 2_756 ?
O12 V003 O12 77.52(13) . 2_756 ?
O6 V003 V004 146.55(12) . . ?
O6 V003 V005 38.01(11) . 2_756 ?
O6 V003 O7 96.48(16) . . ?
O6 V003 O5 97.81(15) . . ?
O6 V003 O12 164.32(14) . . ?
O6 V003 O12 86.81(14) . 2_756 ?
O13 V003 V004 38.79(11) . . ?
O13 V003 V005 145.77(12) . 2_756 ?
O13 V003 O7 97.14(15) . . ?
O13 V003 O5 98.26(15) . . ?
O13 V003 O12 87.90(14) . . ?
O13 V003 O12 165.39(15) . 2_756 ?
O13 V003 O6 107.76(16) . . ?
V003 V004 V002 61.35(2) . . ?
V003 V004 V006 61.60(2) . . ?
V005 V004 V002 60.11(2) . . ?
V005 V004 V003 92.38(3) . . ?
V005 V004 V006 60.31(3) . . ?
V006 V004 V002 90.52(3) . . ?
O12 V004 V002 45.23(8) . . ?
O12 V004 V003 43.34(8) . . ?
O12 V004 V005 49.04(8) . . ?
O12 V004 V006 45.55(8) . . ?
O13 V004 V002 81.16(9) . . ?
O13 V004 V003 30.95(9) . . ?
O13 V004 V005 123.32(9) . . ?
O13 V004 V006 82.32(10) . . ?
O13 V004 O12 74.28(12) . . ?
O2 V004 V002 32.01(10) . . ?
O2 V004 V003 78.27(10) . . ?
O2 V004 V005 83.55(10) . . ?
O2 V004 V006 122.24(10) . . ?
O2 V004 O12 76.69(13) . . ?
O2 V004 O13 82.83(14) . . ?
O16 V004 V002 81.13(11) . . ?
O16 V004 V003 124.80(11) . . ?
O16 V004 V005 32.41(10) . . ?
O16 V004 V006 81.37(11) . . ?
O16 V004 O12 81.46(13) . . ?
O16 V004 O13 155.72(14) . . ?
O16 V004 O2 90.81(15) . . ?
O16 V004 O4 91.41(16) . . ?
O4 V004 V002 122.55(10) . . ?
O4 V004 V003 78.63(11) . . ?
O4 V004 V005 84.16(11) . . ?
O4 V004 V006 32.35(10) . . ?
O4 V004 O12 77.32(13) . . ?
O4 V004 O13 84.27(15) . . ?
O4 V004 O2 153.28(14) . . ?
O3 V004 V002 133.77(15) . . ?
O3 V004 V003 131.13(15) . . ?
O3 V004 V005 136.46(15) . . ?
O3 V004 V006 135.67(15) . . ?
O3 V004 O12 174.37(17) . . ?
O3 V004 O13 100.18(17) . . ?
O3 V004 O2 101.85(18) . . ?
O3 V004 O16 104.05(18) . . ?
O3 V004 O4 103.41(17) . . ?
V002 V005 V003 61.05(2) . 2_756 ?
V004 V005 V002 60.66(3) . . ?
V004 V005 V003 92.17(3) . 2_756 ?
V004 V005 V006 60.14(3) . . ?
V006 V005 V002 90.74(3) . . ?
V006 V005 V003 61.51(2) . 2_756 ?
O12 V005 V002 45.48(8) . . ?
O12 V005 V003 43.50(7) . 2_756 ?
O12 V005 V004 48.67(8) . . ?
O12 V005 V006 45.44(8) . . ?
O6 V005 V002 81.18(10) 2_756 . ?
O6 V005 V003 30.40(9) 2_756 2_756 ?
O6 V005 V004 122.57(9) 2_756 . ?
O6 V005 V006 80.98(9) 2_756 . ?
O6 V005 O12 73.90(12) 2_756 . ?
O8 V005 V002 32.01(10) . . ?
O8 V005 V003 77.68(10) . 2_756 ?
O8 V005 V004 84.48(10) . . ?
O8 V005 V006 122.36(10) . . ?
O8 V005 O12 76.91(13) . . ?
O8 V005 O6 82.99(14) . 2_756 ?
O8 V005 O10 152.68(15) . . ?
O10 V005 V002 122.41(11) . . ?
O10 V005 V003 78.00(10) . 2_756 ?
O10 V005 V004 84.19(10) . . ?
O10 V005 V006 32.13(10) . . ?
O10 V005 O12 76.93(13) . . ?
O10 V005 O6 82.34(14) . 2_756 ?
O16 V005 V002 81.72(11) . . ?
O16 V005 V003 124.72(11) . 2_756 ?
O16 V005 V004 32.55(10) . . ?
O16 V005 V006 81.31(11) . . ?
O16 V005 O12 81.22(13) . . ?
O16 V005 O6 155.12(14) . 2_756 ?
O16 V005 O8 91.92(15) . . ?
O16 V005 O10 91.77(15) . . ?
O9 V005 V002 134.49(15) . . ?
O9 V005 V003 130.69(15) . 2_756 ?
O9 V005 V004 137.13(15) . . ?
O9 V005 V006 134.67(15) . . ?
O9 V005 O12 174.20(17) . . ?
O9 V005 O6 100.29(17) . 2_756 ?
O9 V005 O8 102.57(18) . . ?
O9 V005 O10 102.65(18) . . ?
O9 V005 O16 104.58(18) . . ?
V002 V006 V004 119.64(3) 2_756 . ?
V002 V006 V005 120.04(3) 2_756 . ?
V004 V006 V005 59.55(2) . . ?
O7 V006 V002 39.71(9) 2_756 2_756 ?
O7 V006 V004 124.88(10) 2_756 . ?
O7 V006 V005 87.90(9) 2_756 . ?
O7 V006 O5 76.12(13) 2_756 . ?
O7 V006 O12 76.21(12) 2_756 . ?
O5 V006 V002 39.75(9) . 2_756 ?
O5 V006 V004 87.11(10) . . ?
O5 V006 V005 124.45(10) . . ?
O5 V006 O12 75.53(13) . . ?
O12 V006 V002 84.32(8) . 2_756 ?
O12 V006 V004 48.70(8) . . ?
O12 V006 V005 48.94(8) . . ?
O11 V006 V002 86.58(12) . 2_756 ?
O11 V006 V004 137.88(13) . . ?
O11 V006 V005 137.51(13) . . ?
O11 V006 O7 96.63(15) . 2_756 ?
O11 V006 O5 97.45(15) . . ?
O11 V006 O12 170.90(15) . . ?
O11 V006 O10 103.77(17) . . ?
O11 V006 O4 104.52(17) . . ?
O10 V006 V002 129.48(11) . 2_756 ?
O10 V006 V004 84.98(11) . . ?
O10 V006 V005 33.83(11) . . ?
O10 V006 O7 89.77(14) . 2_756 ?
O10 V006 O5 155.76(15) . . ?
O10 V006 O12 82.07(14) . . ?
O10 V006 O4 96.19(15) . . ?
O4 V006 V002 129.36(11) . 2_756 ?
O4 V006 V004 33.41(11) . . ?
O4 V006 V005 84.29(11) . . ?
O4 V006 O7 155.89(15) . 2_756 ?
O4 V006 O5 89.61(14) . . ?
O4 V006 O12 81.49(14) . . ?
V002 O7 V006 100.48(13) . 2_756 ?
V003 O7 V002 107.10(16) . . ?
V003 O7 V006 107.58(15) . 2_756 ?
V002 O5 V006 100.28(14) 2_756 . ?
V003 O5 V002 107.71(15) . 2_756 ?
V003 O5 V006 107.52(15) . . ?
V002 O12 V004 86.56(11) . . ?
V002 O12 V005 85.66(11) . . ?
V003 O12 V002 93.70(13) . . ?
V003 O12 V002 92.68(12) 2_756 . ?
V003 O12 V003 102.48(13) . 2_756 ?
V003 O12 V004 169.97(16) 2_756 . ?
V003 O12 V004 87.54(11) . . ?
V003 O12 V005 169.83(16) . . ?
V003 O12 V005 87.69(11) 2_756 . ?
V003 O12 V006 93.54(12) 2_756 . ?
V003 O12 V006 93.73(12) . . ?
V004 O12 V005 82.29(10) . . ?
V006 O12 V002 169.06(16) . . ?
V006 O12 V004 85.75(11) . . ?
V006 O12 V005 85.61(11) . . ?
V003 O6 V005 111.59(16) . 2_756 ?
V002 O8 V005 114.57(17) . . ?
V003 O13 V004 110.26(16) . . ?
V002 O1 La1 145.86(18) . 2_756 ?
V006 O11 La1 145.59(19) . . ?
V002 O2 V004 114.20(17) . . ?
V006 O10 V005 114.05(18) . . ?
V005 O16 V004 115.04(17) . . ?
V006 O4 V004 114.24(17) . . ?
La1 O7W H7WA 111.9 . . ?
La1 O7W H7WB 112.5 . . ?
H7WA O7W H7WB 102.0 . . ?
La1 O6W H6WA 110.8 . . ?
La1 O6W H6WB 111.1 . . ?
H6WA O6W H6WB 102.9 . . ?
La1 O1W H1WA 109.6 . . ?
La1 O1W H1WB 109.6 . . ?
H1WA O1W H1WB 104.3 . . ?
La1 O5W H5WA 111.8 . . ?
La1 O5W H5WB 111.8 . . ?
H5WA O5W H5WB 102.3 . . ?
La1 O3W H3WA 127.7 . . ?
La1 O3W H3WB 127.7 . . ?
H3WA O3W H3WB 104.6 . . ?
La1 O4W H4WA 140.3 . . ?
La1 O4W H4WB 107.6 . . ?
H4WA O4W H4WB 104.5 . . ?
La1 O2W H2WA 127.7 . . ?
La1 O2W H2WB 127.7 . . ?
H2WA O2W H2WB 104.7 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
V002 V004 O16 V005 -45.96(17) . . . . ?
V002 V004 O4 V006 9.0(2) . . . . ?
V002 V005 O10 V006 -10.8(2) . . . . ?
V002 V005 O16 V004 46.20(17) . . . . ?
V002 V006 O11 La1 -26.1(3) 2_756 . . . ?
V002 V006 O10 V005 86.32(19) 2_756 . . . ?
V002 V006 O4 V004 -85.30(19) 2_756 . . . ?
V003 V004 O2 V002 -53.72(15) . . . . ?
V003 V004 O16 V005 -0.3(3) . . . . ?
V003 V004 O4 V006 53.89(16) . . . . ?
V003 V005 O8 V002 54.19(15) 2_756 . . . ?
V003 V005 O10 V006 -54.66(15) 2_756 . . . ?
V003 V005 O16 V004 0.3(3) 2_756 . . . ?
V004 V002 O8 V005 38.61(15) . . . . ?
V004 V002 O1 La1 -154.55(19) . . . 2_756 ?
V004 V003 O5 V002 -141.61(12) . . . 2_756 ?
V004 V003 O5 V006 -34.32(12) . . . . ?
V004 V003 O6 V005 179.90(7) . . . 2_756 ?
V004 V005 O8 V002 -39.26(15) . . . . ?
V004 V005 O10 V006 38.82(15) . . . . ?
V004 V006 O11 La1 106.2(3) . . . . ?
V004 V006 O10 V005 -38.49(15) . . . . ?
V005 V002 O1 La1 111.5(3) . . . 2_756 ?
V005 V002 O2 V004 -39.59(15) . . . . ?
V005 V003 O5 V002 33.94(12) 2_756 . . 2_756 ?
V005 V003 O5 V006 141.23(12) 2_756 . . . ?
V005 V003 O13 V004 -179.85(7) 2_756 . . . ?
V005 V004 O2 V002 40.07(15) . . . . ?
V005 V004 O4 V006 -39.73(16) . . . . ?
V005 V006 O11 La1 -158.7(2) . . . . ?
V005 V006 O4 V004 39.36(16) . . . . ?
V006 V002 O8 V005 -85.86(19) 2_756 . . . ?
V006 V002 O1 La1 -21.1(3) 2_756 . . 2_756 ?
V006 V002 O2 V004 85.4(2) 2_756 . . . ?
V006 V004 O2 V002 -8.6(2) . . . . ?
V006 V004 O16 V005 45.92(17) . . . . ?
V006 V005 O8 V002 9.9(2) . . . . ?
V006 V005 O16 V004 -45.83(16) . . . . ?
O7 V002 O8 V005 -31.5(4) . . . . ?
O7 V002 O1 La1 -59.4(3) . . . 2_756 ?
O7 V002 O2 V004 85.56(18) . . . . ?
O7 V003 O5 V002 -52.6(4) . . . 2_756 ?
O7 V003 O5 V006 54.7(4) . . . . ?
O7 V003 O6 V005 80.05(18) . . . 2_756 ?
O7 V003 O13 V004 -81.00(18) . . . . ?
O7 V006 O11 La1 -64.6(3) 2_756 . . . ?
O7 V006 O10 V005 86.57(18) 2_756 . . . ?
O7 V006 O4 V004 -32.4(4) 2_756 . . . ?
O5 V002 O8 V005 -86.10(18) 2_756 . . . ?
O5 V002 O1 La1 17.7(3) 2_756 . . 2_756 ?
O5 V002 O2 V004 31.4(5) 2_756 . . . ?
O5 V003 O6 V005 -78.98(18) . . . 2_756 ?
O5 V003 O13 V004 78.83(18) . . . . ?
O5 V006 O11 La1 12.2(3) . . . . ?
O5 V006 O10 V005 33.0(4) . . . . ?
O5 V006 O4 V004 -85.34(19) . . . . ?
O12 V002 O8 V005 -9.92(16) . . . . ?
O12 V002 O2 V004 9.61(17) . . . . ?
O12 V003 O5 V002 -14.27(14) 2_756 . . 2_756 ?
O12 V003 O5 V002 -93.12(15) . . . 2_756 ?
O12 V003 O5 V006 14.18(14) . . . . ?
O12 V003 O5 V006 93.03(15) 2_756 . . . ?
O12 V003 O6 V005 3.0(7) . . . 2_756 ?
O12 V003 O6 V005 0.82(17) 2_756 . . 2_756 ?
O12 V003 O13 V004 -4.6(7) 2_756 . . . ?
O12 V003 O13 V004 -1.06(17) . . . . ?
O12 V004 O2 V002 -9.30(16) . . . . ?
O12 V004 O16 V005 -0.18(18) . . . . ?
O12 V004 O4 V006 9.55(17) . . . . ?
O12 V005 O8 V002 9.54(16) . . . . ?
O12 V005 O10 V006 -10.05(16) . . . . ?
O12 V005 O16 V004 0.18(18) . . . . ?
O12 V006 O10 V005 10.46(17) . . . . ?
O12 V006 O4 V004 -9.91(17) . . . . ?
O6 V003 O5 V002 71.13(17) . . . 2_756 ?
O6 V003 O5 V006 178.43(15) . . . . ?
O6 V003 O13 V004 179.83(17) . . . . ?
O6 V005 O8 V002 84.58(18) 2_756 . . . ?
O6 V005 O10 V006 -85.22(18) 2_756 . . . ?
O6 V005 O16 V004 -0.8(5) 2_756 . . . ?
O8 V002 O1 La1 109.2(3) . . . 2_756 ?
O8 V002 O2 V004 -71.06(19) . . . . ?
O8 V005 O10 V006 -27.1(4) . . . . ?
O8 V005 O16 V004 76.6(2) . . . . ?
O13 V003 O5 V002 -179.54(16) . . . 2_756 ?
O13 V003 O5 V006 -72.24(17) . . . . ?
O13 V003 O6 V005 179.70(17) . . . 2_756 ?
O13 V004 O2 V002 -84.77(18) . . . . ?
O13 V004 O16 V005 -2.4(5) . . . . ?
O13 V004 O4 V006 84.69(19) . . . . ?
O1 V002 O8 V005 177.12(18) . . . . ?
O1 V002 O2 V004 -176.19(18) . . . . ?
O11 V006 O10 V005 -176.65(18) . . . . ?
O11 V006 O4 V004 177.06(18) . . . . ?
O2 V002 O8 V005 70.52(19) . . . . ?
O2 V002 O1 La1 -151.4(3) . . . 2_756 ?
O2 V004 O16 V005 -76.6(2) . . . . ?
O2 V004 O4 V006 23.3(4) . . . . ?
O10 V005 O8 V002 26.6(4) . . . . ?
O10 V005 O16 V004 -76.3(2) . . . . ?
O10 V006 O11 La1 -156.0(3) . . . . ?
O10 V006 O4 V004 71.1(2) . . . . ?
O16 V004 O2 V002 71.73(19) . . . . ?
O16 V004 O4 V006 -71.4(2) . . . . ?
O16 V005 O8 V002 -70.99(19) . . . . ?
O16 V005 O10 V006 70.51(19) . . . . ?
O4 V004 O2 V002 -23.0(4) . . . . ?
O4 V004 O16 V005 76.8(2) . . . . ?
O4 V006 O11 La1 103.8(3) . . . . ?
O4 V006 O10 V005 -70.0(2) . . . . ?
O9 V005 O8 V002 -176.4(2) . . . . ?
O9 V005 O10 V006 175.9(2) . . . . ?
O9 V005 O16 V004 -179.9(2) . . . . ?
O3 V004 O2 V002 176.3(2) . . . . ?
O3 V004 O16 V005 -179.0(2) . . . . ?
O3 V004 O4 V006 -176.2(2) . . . . ?

_smtbx_masks_special_details     ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 0.500 0.000 0.000 151.1 32.3 ?

_smtbx_masks_void_probe_radius   1.2
_smtbx_masks_void_truncation_radius 1.2
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.535
_oxdiff_exptl_absorpt_empirical_full_min 0.540
_oxdiff_twin_integration_method  simultaneous
_oxdiff_twin_items               2
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_oxdiff_twin_reflns_isolated
_oxdiff_twin_reflns_overlapped
_twin_individual_twin_lattice_type
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.6294(11) 13599 23749 ref 1.0000 0.0000 0.0000 0.0000 1.0000 0.0000 0.0000
0.0000 1.0000
2 0.3706(11) 13312 23749 nmt 1.0090 0.0179 0.0315 -0.0041 0.9987 -0.0023
-0.0308 -0.0083 0.9932

_twin_special_details            
;
Component 2 rotated by 1.7539° 
around [-0.11 0.88 -0.47] (reciprocal) or [0.00 0.99 -0.13] (direct)
;
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_jaso040_sq
_database_code_depnum_ccdc_archive 'CCDC 2341648'
loop_
_audit_author_name
_audit_author_address
'Robert Gyepes'
;Charles University
Czech Republic
;
_audit_update_record             
;
2024-03-20 deposited with the CCDC.	2024-12-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2019/3
_shelx_SHELXL_version_number     2019/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'La12 O184 V46 [+ solvent]'
_chemical_formula_sum            'H96 La12 O232 V46'
_chemical_formula_weight         7818.92

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_H-M_alt        'P n m a'
_space_group_name_Hall           '-P 2ac 2n'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   18.7636(6)
_cell_length_b                   24.2176(8)
_cell_length_c                   23.0563(8)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     10477.0(6)
_cell_formula_units_Z            2
_cell_measurement_temperature    120(2)
_cell_measurement_reflns_used    9055
_cell_measurement_theta_min      2.1885
_cell_measurement_theta_max      28.3466

_exptl_crystal_description       needle
_exptl_crystal_colour            orange
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.479
_exptl_crystal_F_000             7388
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.361
_exptl_crystal_size_mid          0.105
_exptl_crystal_size_min          0.090
_exptl_absorpt_coefficient_mu    4.459
_shelx_estimated_absorpt_T_min   0.296
_shelx_estimated_absorpt_T_max   0.690
_exptl_absorpt_correction_type   Multi-Scan
_exptl_absorpt_process_details   
;
Krause, L., Herbst-Irmer, R., Sheldrick, G. M., Stalke, D. (2015).
"Comparison of silver and molybdenum microfocus X-ray sources for
single-crystal structure determination"
J. Appl. Cryst. 48, 3-10.
doi:10.1107/S1600576714022985
;
_exptl_absorpt_correction_T_min  0.33
_exptl_absorpt_correction_T_max  0.47
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      120(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker D8 VENTURE'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            125770
_diffrn_reflns_av_unetI/netI     0.0402
_diffrn_reflns_av_R_equivalents  0.0825
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_k_min       -31
_diffrn_reflns_limit_k_max       31
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_theta_min         2.073
_diffrn_reflns_theta_max         27.492
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             12307
_reflns_number_gt                9674
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2019/2 (Sheldrick, 2019)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0410P)²+284.8484P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         12307
_refine_ls_number_parameters     571
_refine_ls_number_restraints     12
_refine_ls_R_factor_all          0.0902
_refine_ls_R_factor_gt           0.0691
_refine_ls_wR_factor_ref         0.1632
_refine_ls_wR_factor_gt          0.1516
_refine_ls_goodness_of_fit_ref   1.092
_refine_ls_restrained_S_all      1.093
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.74826(3) 0.40625(2) 0.38316(3) 0.02549(14) Uani 1 1 d . . . . .
La2 La 0.52939(4) 0.250000 0.16114(3) 0.01814(16) Uani 1 2 d S T P . .
La3 La 0.33963(3) 0.09395(2) 0.40309(3) 0.02650(14) Uani 1 1 d . . . . .
La4 La 0.56299(6) 0.250000 0.62916(4) 0.0423(2) Uani 1 2 d S T P . .
V1 V 0.91698(10) 0.50696(9) 0.40551(9) 0.0391(5) Uani 1 1 d . . . . .
V2 V 1.05832(11) 0.56625(9) 0.37701(10) 0.0444(5) Uani 1 1 d . . . . .
V3 V 1.08442(9) 0.59007(8) 0.50751(9) 0.0363(5) Uani 1 1 d . . . . .
V4 V 0.93886(9) 0.53228(8) 0.53796(9) 0.0360(5) Uani 1 1 d . . . . .
V5 V 0.94465(10) 0.62601(9) 0.44806(10) 0.0423(5) Uani 1 1 d . . . . .
V6 V 0.63683(8) 0.18464(7) 0.48739(7) 0.0223(3) Uani 1 1 d . . . . .
V7 V 0.71244(10) 0.250000 0.38718(9) 0.0145(4) Uani 1 2 d S T P . .
V8 V 0.62098(7) 0.31568(6) 0.29567(6) 0.0131(3) Uani 1 1 d . . . . .
V9 V 0.54452(8) 0.38135(6) 0.39552(7) 0.0194(3) Uani 1 1 d . . . . .
V10 V 0.46643(8) 0.31596(7) 0.49596(7) 0.0215(3) Uani 1 1 d . . . . .
V11 V 0.54418(10) 0.250000 0.39696(9) 0.0135(4) Uani 1 2 d S T P . .
V12 V 0.45380(7) 0.31488(6) 0.30376(6) 0.0152(3) Uani 1 1 d . . . . .
V13 V 0.37603(10) 0.250000 0.40493(9) 0.0158(4) Uani 1 2 d S T P . .
O1 O 0.8538(4) 0.4748(3) 0.3721(3) 0.040(2) Uani 1 1 d . . . . .
O2 O 0.9814(4) 0.5239(4) 0.3502(4) 0.043(2) Uani 1 1 d . . . . .
O3 O 1.1201(4) 0.5927(3) 0.4350(4) 0.044(2) Uani 1 1 d . . . . .
O4 O 1.0244(4) 0.5592(3) 0.5712(3) 0.0376(19) Uani 1 1 d . . . . .
O5 O 0.8825(4) 0.4897(3) 0.4852(3) 0.0348(18) Uani 1 1 d . . . . .
O6 O 0.8822(4) 0.5760(4) 0.4119(4) 0.046(2) Uani 1 1 d . . . . .
O7 O 1.0203(4) 0.6452(3) 0.4976(4) 0.041(2) Uani 1 1 d . . . . .
O8 O 1.1041(5) 0.5770(4) 0.3193(4) 0.057(3) Uani 1 1 d . . . . .
O9 O 1.1474(4) 0.6167(3) 0.5468(4) 0.0356(18) Uani 1 1 d . . . . .
O10 O 0.9005(4) 0.5088(3) 0.6001(4) 0.042(2) Uani 1 1 d . . . . .
O11 O 1.0015(5) 0.6272(4) 0.3837(4) 0.051(2) Uani 1 1 d . . . . .
O12 O 0.9008(4) 0.5938(3) 0.5233(4) 0.040(2) Uani 1 1 d . . . . .
O13 O 0.9019(5) 0.6829(4) 0.4444(4) 0.055(2) Uani 1 1 d . . . . .
O14 O 0.7659(3) 0.3039(3) 0.3836(3) 0.0205(13) Uani 1 1 d . . . . .
O15 O 0.6133(3) 0.4231(3) 0.3924(3) 0.0236(14) Uani 1 1 d . . . . .
O16 O 0.6830(3) 0.3631(3) 0.3005(3) 0.0201(13) Uani 1 1 d . . . . .
O17 O 0.7423(4) 0.4835(3) 0.4575(4) 0.040(2) Uani 1 1 d . . . . .
O18 O 0.8384(4) 0.3810(4) 0.3043(4) 0.046(2) Uani 1 1 d . . . . .
O19 O 0.7127(5) 0.4818(4) 0.3114(6) 0.082(4) Uani 1 1 d . . . . .
O20 O 0.6780(4) 0.250000 0.3084(3) 0.0111(16) Uani 1 2 d S T P . .
O21 O 0.6912(4) 0.250000 0.4697(4) 0.0184(18) Uani 1 2 d S T P . .
O22 O 0.6167(3) 0.1937(2) 0.3922(3) 0.0169(12) Uani 1 1 d . . . . .
O23 O 0.6336(3) 0.1907(3) 0.5585(3) 0.0307(16) Uani 1 1 d . . . . .
O24 O 0.6969(3) 0.1360(3) 0.4752(3) 0.0257(15) Uani 1 1 d . . . . .
O25 O 0.5373(4) 0.250000 0.3142(4) 0.0118(16) Uani 1 2 d S TU P . .
O26 O 0.4720(3) 0.1933(2) 0.4000(3) 0.0161(12) Uani 1 1 d . . . . .
O27 O 0.4088(4) 0.250000 0.4834(4) 0.0198(19) Uani 1 2 d S T P . .
O28 O 0.3979(4) 0.250000 0.3235(4) 0.0187(18) Uani 1 2 d S T P . .
O29 O 0.3924(3) 0.3618(3) 0.3147(3) 0.0228(14) Uani 1 1 d . . . . .
O30 O 0.4564(3) 0.3077(3) 0.2328(3) 0.0197(13) Uani 1 1 d . . . . .
O31 O 0.6065(3) 0.3091(2) 0.2261(3) 0.0164(12) Uani 1 1 d . . . . .
O32 O 0.6584(5) 0.250000 0.1249(5) 0.055(4) Uani 1 2 d S T P . .
O33 O 0.5254(6) 0.250000 0.0491(4) 0.043(3) Uani 1 2 d S T P . .
O34 O 0.4008(7) 0.250000 0.1248(7) 0.090(6) Uani 1 2 d S T P . .
O35 O 0.5251(8) 0.1506(4) 0.1284(5) 0.085(4) Uani 1 1 d . . . . .
O36 O 0.4809(4) 0.3089(3) 0.5664(3) 0.0317(16) Uani 1 1 d . . . . .
O37 O 0.4040(3) 0.3641(3) 0.4906(3) 0.0254(15) Uani 1 1 d . . . . .
O38 O 0.5507(4) 0.250000 0.4784(4) 0.0202(19) Uani 1 2 d S T P . .
O39 O 0.3223(3) 0.1964(3) 0.4069(3) 0.0226(14) Uani 1 1 d . . . . .
O40 O 0.2357(5) 0.1215(4) 0.3368(4) 0.054(2) Uani 1 1 d . . . . .
O41 O 0.3655(5) 0.0197(4) 0.3272(4) 0.054(2) Uani 1 1 d . . . . .
O42 O 0.2459(4) 0.0182(4) 0.4035(4) 0.049(2) Uani 1 1 d . . . . .
O43 O 0.3716(4) 0.0159(3) 0.4743(4) 0.0386(19) Uani 1 1 d . . . . .
O44 O 0.2463(4) 0.1177(4) 0.4807(5) 0.063(3) Uani 1 1 d . . . . .
O45 O 0.4366(9) 0.250000 0.6746(7) 0.081(5) Uani 1 2 d S T P . .
O46 O 0.5676(14) 0.250000 0.7396(8) 0.116(8) Uani 1 2 d S T P . .
O47 O 0.5638(6) 0.3505(5) 0.6659(4) 0.066(3) Uani 1 1 d . . . . .
O48 O 0.9999(4) 0.5420(3) 0.4620(3) 0.0350(18) Uani 1 1 d . . . . .
O49 O 0.4747(3) 0.4227(3) 0.3987(3) 0.0248(14) Uani 1 1 d . . . . .
O50 O 0.5506(3) 0.3596(3) 0.4763(3) 0.0209(13) Uani 1 1 d . . . . .
O51 O 0.5382(3) 0.3591(2) 0.3152(3) 0.0170(12) Uani 1 1 d . . . . .
O52 O 0.6806(12) 0.250000 0.6636(10) 0.119(7) Uani 1 2 d S TU P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 O16 2.494(6) . ?
La1 O14 2.500(6) . ?
La1 O17 2.540(7) . ?
La1 O24 2.545(7) 7_565 ?
La1 O19 2.555(11) . ?
La1 O18 2.557(8) . ?
La1 O15 2.575(6) . ?
La1 O1 2.596(7) . ?
La1 O9 2.598(8) 5_766 ?
La2 O35 2.525(10) . ?
La2 O35 2.525(10) 7_565 ?
La2 O31 2.526(6) 7_565 ?
La2 O31 2.526(6) . ?
La2 O34 2.555(13) . ?
La2 O32 2.561(10) . ?
La2 O30 2.561(6) 7_565 ?
La2 O30 2.562(6) . ?
La2 O33 2.585(10) . ?
La3 O39 2.504(7) . ?
La3 O29 2.507(6) 7_565 ?
La3 O42 2.542(8) . ?
La3 O41 2.556(9) . ?
La3 O37 2.562(7) 7_565 ?
La3 O40 2.566(9) . ?
La3 O49 2.567(6) 7_565 ?
La3 O44 2.570(9) . ?
La3 O43 2.574(8) . ?
La4 O52 2.35(2) . ?
La4 O23 2.544(7) . ?
La4 O23 2.544(7) 7_565 ?
La4 O46 2.547(19) . ?
La4 O36 2.550(8) . ?
La4 O36 2.550(8) 7_565 ?
La4 O47 2.577(11) . ?
La4 O47 2.577(11) 7_565 ?
La4 O45 2.592(15) . ?
V1 O1 1.615(7) . ?
V1 O6 1.802(9) . ?
V1 O2 1.805(8) . ?
V1 O5 1.992(8) . ?
V1 O4 2.017(9) 5_766 ?
V1 O48 2.200(7) . ?
V1 V2 3.087(3) . ?
V1 V5 3.089(3) . ?
V1 V3 3.090(3) 5_766 ?
V2 O8 1.605(9) . ?
V2 O11 1.827(10) . ?
V2 O2 1.874(7) . ?
V2 O3 1.881(8) . ?
V2 O10 2.045(10) 5_766 ?
V2 O48 2.322(8) . ?
V2 V5 3.054(3) . ?
V2 V4 3.089(3) 5_766 ?
V2 V3 3.102(3) . ?
V3 O9 1.623(7) . ?
V3 O3 1.801(8) . ?
V3 O7 1.813(9) . ?
V3 O4 1.997(8) . ?
V3 O5 2.036(8) 5_766 ?
V3 O48 2.229(7) . ?
V3 V5 3.084(3) . ?
V4 O12 1.687(9) . ?
V4 O10 1.701(8) . ?
V4 O4 1.894(7) . ?
V4 O5 1.914(7) . ?
V4 O48 2.105(7) . ?
V4 O48 2.135(8) 5_766 ?
V4 V5 3.076(3) . ?
V5 O13 1.596(10) . ?
V5 O11 1.827(9) . ?
V5 O6 1.880(8) . ?
V5 O7 1.881(8) . ?
V5 O12 2.073(9) . ?
V5 O48 2.305(9) . ?
V6 O23 1.647(7) . ?
V6 O24 1.655(7) . ?
V6 O21 1.927(5) . ?
V6 O50 1.957(6) 7_565 ?
V6 O22 2.238(6) . ?
V6 O38 2.272(6) . ?
V7 O14 1.649(6) . ?
V7 O14 1.649(6) 7_565 ?
V7 O20 1.929(8) . ?
V7 O21 1.943(9) . ?
V7 O22 2.259(6) . ?
V7 O22 2.259(6) 7_565 ?
V8 O31 1.635(6) . ?
V8 O16 1.639(6) . ?
V8 O51 1.929(6) . ?
V8 O20 1.939(5) . ?
V8 O22 2.238(6) 7_565 ?
V8 O25 2.275(5) . ?
V9 O15 1.641(6) . ?
V9 O49 1.651(6) . ?
V9 O51 1.933(6) . ?
V9 O50 1.939(7) . ?
V9 O26 2.265(6) 7_565 ?
V9 O22 2.267(6) 7_565 ?
V10 O36 1.656(8) . ?
V10 O37 1.657(7) . ?
V10 O27 1.951(5) . ?
V10 O50 1.954(6) . ?
V10 O26 2.225(6) 7_565 ?
V10 O38 2.284(6) . ?
V11 O38 1.881(9) . ?
V11 O25 1.913(8) . ?
V11 O26 1.929(6) . ?
V11 O26 1.929(6) 7_565 ?
V11 O22 1.929(6) . ?
V11 O22 1.929(6) 7_565 ?
V12 O29 1.637(6) . ?
V12 O30 1.646(6) . ?
V12 O51 1.929(6) . ?
V12 O28 1.943(5) . ?
V12 O25 2.233(5) . ?
V12 O26 2.255(6) 7_565 ?
V13 O39 1.644(6) 7_565 ?
V13 O39 1.644(6) . ?
V13 O27 1.911(9) . ?
V13 O28 1.921(9) . ?
V13 O26 2.267(6) . ?
V13 O26 2.267(6) 7_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 La1 O14 69.68(19) . . ?
O16 La1 O17 143.4(2) . . ?
O14 La1 O17 137.2(3) . . ?
O16 La1 O24 106.42(19) . 7_565 ?
O14 La1 O24 69.5(2) . 7_565 ?
O17 La1 O24 73.6(2) . 7_565 ?
O16 La1 O19 71.2(3) . . ?
O14 La1 O19 138.3(3) . . ?
O17 La1 O19 84.1(4) . . ?
O24 La1 O19 136.8(3) 7_565 . ?
O16 La1 O18 71.4(2) . . ?
O14 La1 O18 71.2(2) . . ?
O17 La1 O18 133.2(2) . . ?
O24 La1 O18 138.3(3) 7_565 . ?
O19 La1 O18 83.3(3) . . ?
O16 La1 O15 69.3(2) . . ?
O14 La1 O15 106.7(2) . . ?
O17 La1 O15 77.5(2) . . ?
O24 La1 O15 67.8(2) 7_565 . ?
O19 La1 O15 71.6(3) . . ?
O18 La1 O15 138.4(3) . . ?
O16 La1 O1 124.5(2) . . ?
O14 La1 O1 122.2(2) . . ?
O17 La1 O1 68.2(2) . . ?
O24 La1 O1 128.9(2) 7_565 . ?
O19 La1 O1 71.2(3) . . ?
O18 La1 O1 65.1(2) . . ?
O15 La1 O1 131.1(2) . . ?
O16 La1 O9 139.0(2) . 5_766 ?
O14 La1 O9 71.7(2) . 5_766 ?
O17 La1 O9 76.8(2) . 5_766 ?
O24 La1 O9 71.4(2) 7_565 5_766 ?
O19 La1 O9 138.8(3) . 5_766 ?
O18 La1 O9 83.8(3) . 5_766 ?
O15 La1 O9 136.4(2) . 5_766 ?
O1 La1 O9 67.9(3) . 5_766 ?
O35 La2 O35 145.0(5) . 7_565 ?
O35 La2 O31 69.8(3) . 7_565 ?
O35 La2 O31 137.4(3) 7_565 7_565 ?
O35 La2 O31 137.4(3) . . ?
O35 La2 O31 69.8(3) 7_565 . ?
O31 La2 O31 69.0(3) 7_565 . ?
O35 La2 O34 82.6(3) . . ?
O35 La2 O34 82.6(3) 7_565 . ?
O31 La2 O34 137.3(3) 7_565 . ?
O31 La2 O34 137.3(2) . . ?
O35 La2 O32 86.1(3) . . ?
O35 La2 O32 86.1(3) 7_565 . ?
O31 La2 O32 69.7(2) 7_565 . ?
O31 La2 O32 69.7(2) . . ?
O34 La2 O32 141.8(5) . . ?
O35 La2 O30 69.9(3) . 7_565 ?
O35 La2 O30 134.1(3) 7_565 7_565 ?
O31 La2 O30 67.34(19) 7_565 7_565 ?
O31 La2 O30 103.46(19) . 7_565 ?
O34 La2 O30 72.9(3) . 7_565 ?
O32 La2 O30 135.8(2) . 7_565 ?
O35 La2 O30 134.1(3) . . ?
O35 La2 O30 69.9(3) 7_565 . ?
O31 La2 O30 103.46(19) 7_565 . ?
O31 La2 O30 67.34(19) . . ?
O34 La2 O30 72.9(3) . . ?
O32 La2 O30 135.8(2) . . ?
O30 La2 O30 66.1(3) 7_565 . ?
O35 La2 O33 72.5(3) . . ?
O35 La2 O33 72.5(3) 7_565 . ?
O31 La2 O33 127.5(2) 7_565 . ?
O31 La2 O33 127.5(2) . . ?
O34 La2 O33 69.2(5) . . ?
O32 La2 O33 72.6(4) . . ?
O30 La2 O33 129.0(2) 7_565 . ?
O30 La2 O33 129.0(2) . . ?
O39 La3 O29 69.8(2) . 7_565 ?
O39 La3 O42 128.7(2) . . ?
O29 La3 O42 125.8(3) 7_565 . ?
O39 La3 O41 138.2(3) . . ?
O29 La3 O41 70.7(2) 7_565 . ?
O42 La3 O41 68.0(3) . . ?
O39 La3 O37 68.9(2) . 7_565 ?
O29 La3 O37 106.5(2) 7_565 7_565 ?
O42 La3 O37 127.6(3) . 7_565 ?
O41 La3 O37 136.8(3) . 7_565 ?
O39 La3 O40 70.4(3) . . ?
O29 La3 O40 72.8(3) 7_565 . ?
O42 La3 O40 70.4(3) . . ?
O41 La3 O40 85.4(3) . . ?
O37 La3 O40 136.4(3) 7_565 . ?
O39 La3 O49 106.55(19) . 7_565 ?
O29 La3 O49 69.2(2) 7_565 7_565 ?
O42 La3 O49 124.7(2) . 7_565 ?
O41 La3 O49 71.0(3) . 7_565 ?
O37 La3 O49 68.2(2) 7_565 7_565 ?
O40 La3 O49 140.1(3) . 7_565 ?
O39 La3 O44 70.5(3) . . ?
O29 La3 O44 137.7(3) 7_565 . ?
O42 La3 O44 71.8(3) . . ?
O41 La3 O44 139.8(3) . . ?
O37 La3 O44 71.5(3) 7_565 . ?
O40 La3 O44 80.8(3) . . ?
O49 La3 O44 137.3(3) 7_565 . ?
O39 La3 O43 137.3(2) . . ?
O29 La3 O43 137.8(2) 7_565 . ?
O42 La3 O43 68.2(3) . . ?
O41 La3 O43 82.9(3) . . ?
O37 La3 O43 71.3(2) 7_565 . ?
O40 La3 O43 138.4(3) . . ?
O49 La3 O43 71.4(2) 7_565 . ?
O44 La3 O43 83.0(3) . . ?
O52 La4 O23 74.2(5) . . ?
O52 La4 O23 74.2(5) . 7_565 ?
O23 La4 O23 68.7(3) . 7_565 ?
O52 La4 O46 68.3(8) . . ?
O23 La4 O46 128.5(4) . . ?
O23 La4 O46 128.5(4) 7_565 . ?
O52 La4 O36 139.5(3) . . ?
O23 La4 O36 105.5(2) . . ?
O23 La4 O36 68.6(2) 7_565 . ?
O46 La4 O36 126.0(4) . . ?
O52 La4 O36 139.5(3) . 7_565 ?
O23 La4 O36 68.6(2) . 7_565 ?
O23 La4 O36 105.5(2) 7_565 7_565 ?
O46 La4 O36 126.0(4) . 7_565 ?
O36 La4 O36 68.0(3) . 7_565 ?
O52 La4 O47 83.3(3) . . ?
O23 La4 O47 137.7(3) . . ?
O23 La4 O47 71.0(3) 7_565 . ?
O46 La4 O47 70.8(2) . . ?
O36 La4 O47 70.2(3) . . ?
O36 La4 O47 135.9(3) 7_565 . ?
O52 La4 O47 83.3(3) . 7_565 ?
O23 La4 O47 71.0(3) . 7_565 ?
O23 La4 O47 137.7(3) 7_565 7_565 ?
O46 La4 O47 70.8(2) . 7_565 ?
O36 La4 O47 135.9(3) . 7_565 ?
O36 La4 O47 70.2(3) 7_565 7_565 ?
O47 La4 O47 141.6(5) . 7_565 ?
O52 La4 O45 136.3(7) . . ?
O23 La4 O45 137.3(3) . . ?
O23 La4 O45 137.3(3) 7_565 . ?
O46 La4 O45 68.1(7) . . ?
O36 La4 O45 71.1(4) . . ?
O36 La4 O45 71.1(4) 7_565 . ?
O47 La4 O45 82.7(3) . . ?
O47 La4 O45 82.7(3) 7_565 . ?
O1 V1 O6 102.8(4) . . ?
O1 V1 O2 105.3(4) . . ?
O6 V1 O2 95.1(4) . . ?
O1 V1 O5 95.8(4) . . ?
O6 V1 O5 90.1(4) . . ?
O2 V1 O5 156.5(4) . . ?
O1 V1 O4 98.3(4) . 5_766 ?
O6 V1 O4 156.0(4) . 5_766 ?
O2 V1 O4 90.2(4) . 5_766 ?
O5 V1 O4 76.4(3) . 5_766 ?
O1 V1 O48 171.2(4) . . ?
O6 V1 O48 81.3(3) . . ?
O2 V1 O48 81.8(3) . . ?
O5 V1 O48 76.4(3) . . ?
O4 V1 O48 76.3(3) 5_766 . ?
O1 V1 V2 138.9(3) . . ?
O6 V1 V2 84.1(2) . . ?
O2 V1 V2 33.7(2) . . ?
O5 V1 V2 125.0(2) . . ?
O4 V1 V2 87.6(2) 5_766 . ?
O48 V1 V2 48.6(2) . . ?
O1 V1 V5 136.5(3) . . ?
O6 V1 V5 33.8(2) . . ?
O2 V1 V5 84.2(3) . . ?
O5 V1 V5 87.6(2) . . ?
O4 V1 V5 124.4(2) 5_766 . ?
O48 V1 V5 48.2(2) . . ?
V2 V1 V5 59.27(6) . . ?
O1 V1 V3 86.4(3) . 5_766 ?
O6 V1 V3 130.5(3) . 5_766 ?
O2 V1 V3 129.6(3) . 5_766 ?
O5 V1 V3 40.4(2) . 5_766 ?
O4 V1 V3 39.4(2) 5_766 5_766 ?
O48 V1 V3 85.1(2) . 5_766 ?
V2 V1 V3 119.95(9) . 5_766 ?
V5 V1 V3 120.34(9) . 5_766 ?
O8 V2 O11 104.6(5) . . ?
O8 V2 O2 103.1(4) . . ?
O11 V2 O2 91.2(4) . . ?
O8 V2 O3 101.8(4) . . ?
O11 V2 O3 91.4(4) . . ?
O2 V2 O3 153.4(4) . . ?
O8 V2 O10 98.9(5) . 5_766 ?
O11 V2 O10 156.5(4) . 5_766 ?
O2 V2 O10 83.6(4) . 5_766 ?
O3 V2 O10 83.5(4) . 5_766 ?
O8 V2 O48 173.6(5) . . ?
O11 V2 O48 81.8(4) . . ?
O2 V2 O48 77.1(3) . . ?
O3 V2 O48 77.1(3) . . ?
O10 V2 O48 74.7(3) 5_766 . ?
O8 V2 V5 137.9(4) . . ?
O11 V2 V5 33.3(3) . . ?
O2 V2 V5 84.2(2) . . ?
O3 V2 V5 83.5(2) . . ?
O10 V2 V5 123.2(2) 5_766 . ?
O48 V2 V5 48.5(2) . . ?
O8 V2 V1 135.4(3) . . ?
O11 V2 V1 81.7(3) . . ?
O2 V2 V1 32.3(2) . . ?
O3 V2 V1 122.4(3) . . ?
O10 V2 V1 81.7(2) 5_766 . ?
O48 V2 V1 45.32(17) . . ?
V5 V2 V1 60.41(6) . . ?
O8 V2 V4 129.9(4) . 5_766 ?
O11 V2 V4 125.5(3) . 5_766 ?
O2 V2 V4 78.5(3) . 5_766 ?
O3 V2 V4 78.5(3) . 5_766 ?
O10 V2 V4 31.0(2) 5_766 5_766 ?
O48 V2 V4 43.7(2) . 5_766 ?
V5 V2 V4 92.15(8) . 5_766 ?
V1 V2 V4 61.33(7) . 5_766 ?
O8 V2 V3 133.6(3) . . ?
O11 V2 V3 82.0(3) . . ?
O2 V2 V3 122.9(3) . . ?
O3 V2 V3 31.8(2) . . ?
O10 V2 V3 81.7(2) 5_766 . ?
O48 V2 V3 45.79(17) . . ?
V5 V2 V3 60.13(7) . . ?
V1 V2 V3 90.90(7) . . ?
V4 V2 V3 61.66(7) 5_766 . ?
O9 V3 O3 103.5(4) . . ?
O9 V3 O7 105.1(4) . . ?
O3 V3 O7 96.0(4) . . ?
O9 V3 O4 98.6(4) . . ?
O3 V3 O4 154.9(3) . . ?
O7 V3 O4 89.6(4) . . ?
O9 V3 O5 96.2(4) . 5_766 ?
O3 V3 O5 89.8(4) . 5_766 ?
O7 V3 O5 155.8(3) . 5_766 ?
O4 V3 O5 75.9(3) . 5_766 ?
O9 V3 O48 171.2(4) . . ?
O3 V3 O48 81.2(3) . . ?
O7 V3 O48 81.6(3) . . ?
O4 V3 O48 75.5(3) . . ?
O5 V3 O48 76.2(3) 5_766 . ?
O9 V3 V5 139.0(3) . . ?
O3 V3 V5 83.9(3) . . ?
O7 V3 V5 34.1(2) . . ?
O4 V3 V5 87.3(3) . . ?
O5 V3 V5 124.3(2) 5_766 . ?
O48 V3 V5 48.2(2) . . ?
O9 V3 V1 86.9(3) . 5_766 ?
O3 V3 V1 129.2(3) . 5_766 ?
O7 V3 V1 129.5(3) . 5_766 ?
O4 V3 V1 39.9(2) . 5_766 ?
O5 V3 V1 39.4(2) 5_766 5_766 ?
O48 V3 V1 84.4(2) . 5_766 ?
V5 V3 V1 119.73(8) . 5_766 ?
O9 V3 V2 136.9(3) . . ?
O3 V3 V2 33.4(2) . . ?
O7 V3 V2 84.9(3) . . ?
O4 V3 V2 123.7(2) . . ?
O5 V3 V2 87.3(2) 5_766 . ?
O48 V3 V2 48.3(2) . . ?
V5 V3 V2 59.16(7) . . ?
V1 V3 V2 119.13(8) 5_766 . ?
O12 V4 O10 106.5(4) . . ?
O12 V4 O4 97.8(4) . . ?
O10 V4 O4 97.6(4) . . ?
O12 V4 O5 96.6(4) . . ?
O10 V4 O5 97.0(3) . . ?
O4 V4 O5 155.7(3) . . ?
O12 V4 O48 88.0(4) . . ?
O10 V4 O48 165.5(4) . . ?
O4 V4 O48 80.7(3) . . ?
O5 V4 O48 80.3(3) . . ?
O12 V4 O48 166.6(4) . 5_766 ?
O10 V4 O48 86.9(4) . 5_766 ?
O4 V4 O48 80.5(3) . 5_766 ?
O5 V4 O48 81.0(3) . 5_766 ?
O48 V4 O48 78.6(4) . 5_766 ?
O12 V4 V5 39.5(3) . . ?
O10 V4 V5 146.0(3) . . ?
O4 V4 V5 89.4(3) . . ?
O5 V4 V5 89.4(3) . . ?
O48 V4 V5 48.5(2) . . ?
O48 V4 V5 127.1(2) 5_766 . ?
O12 V4 V2 144.7(3) . 5_766 ?
O10 V4 V2 38.2(3) . 5_766 ?
O4 V4 V2 89.7(3) . 5_766 ?
O5 V4 V2 89.8(3) . 5_766 ?
O48 V4 V2 127.2(2) . 5_766 ?
O48 V4 V2 48.7(2) 5_766 5_766 ?
V5 V4 V2 175.76(8) . 5_766 ?
O13 V5 O11 103.7(5) . . ?
O13 V5 O6 102.6(4) . . ?
O11 V5 O6 90.8(4) . . ?
O13 V5 O7 101.4(4) . . ?
O11 V5 O7 92.8(4) . . ?
O6 V5 O7 154.1(4) . . ?
O13 V5 O12 99.8(4) . . ?
O11 V5 O12 156.5(4) . . ?
O6 V5 O12 83.2(3) . . ?
O7 V5 O12 83.3(3) . . ?
O13 V5 O48 174.1(4) . . ?
O11 V5 O48 82.2(4) . . ?
O6 V5 O48 77.0(3) . . ?
O7 V5 O48 78.1(3) . . ?
O12 V5 O48 74.3(3) . . ?
O13 V5 V2 137.0(4) . . ?
O11 V5 V2 33.3(3) . . ?
O6 V5 V2 83.9(2) . . ?
O7 V5 V2 85.2(2) . . ?
O12 V5 V2 123.3(2) . . ?
O48 V5 V2 48.93(19) . . ?
O13 V5 V4 130.9(4) . . ?
O11 V5 V4 125.4(3) . . ?
O6 V5 V4 78.6(3) . . ?
O7 V5 V4 78.5(3) . . ?
O12 V5 V4 31.2(2) . . ?
O48 V5 V4 43.16(18) . . ?
V2 V5 V4 92.09(8) . . ?
O13 V5 V3 134.0(3) . . ?
O11 V5 V3 82.5(3) . . ?
O6 V5 V3 123.1(3) . . ?
O7 V5 V3 32.7(2) . . ?
O12 V5 V3 81.9(2) . . ?
O48 V5 V3 46.11(17) . . ?
V2 V5 V3 60.71(7) . . ?
V4 V5 V3 61.47(7) . . ?
O13 V5 V1 134.7(3) . . ?
O11 V5 V1 81.6(3) . . ?
O6 V5 V1 32.2(3) . . ?
O7 V5 V1 123.4(3) . . ?
O12 V5 V1 81.3(2) . . ?
O48 V5 V1 45.30(17) . . ?
V2 V5 V1 60.32(6) . . ?
V4 V5 V1 61.27(7) . . ?
V3 V5 V1 91.19(8) . . ?
O23 V6 O24 105.0(3) . . ?
O23 V6 O21 99.0(4) . . ?
O24 V6 O21 100.9(3) . . ?
O23 V6 O50 98.5(3) . 7_565 ?
O24 V6 O50 98.7(3) . 7_565 ?
O21 V6 O50 149.3(3) . 7_565 ?
O23 V6 O22 164.0(3) . . ?
O24 V6 O22 91.0(3) . . ?
O21 V6 O22 78.5(3) . . ?
O50 V6 O22 77.6(2) 7_565 . ?
O23 V6 O38 90.1(3) . . ?
O24 V6 O38 164.9(3) . . ?
O21 V6 O38 77.6(3) . . ?
O50 V6 O38 77.4(2) 7_565 . ?
O22 V6 O38 73.8(3) . . ?
O14 V7 O14 104.7(4) . 7_565 ?
O14 V7 O20 99.0(3) . . ?
O14 V7 O20 99.0(3) 7_565 . ?
O14 V7 O21 100.0(3) . . ?
O14 V7 O21 100.0(3) 7_565 . ?
O20 V7 O21 148.6(3) . . ?
O14 V7 O22 164.8(3) . . ?
O14 V7 O22 90.5(3) 7_565 . ?
O20 V7 O22 77.4(2) . . ?
O21 V7 O22 77.7(3) . . ?
O14 V7 O22 90.5(3) . 7_565 ?
O14 V7 O22 164.8(3) 7_565 7_565 ?
O20 V7 O22 77.4(2) . 7_565 ?
O21 V7 O22 77.7(3) . 7_565 ?
O22 V7 O22 74.3(3) . 7_565 ?
O31 V8 O16 104.7(3) . . ?
O31 V8 O51 98.5(3) . . ?
O16 V8 O51 100.1(3) . . ?
O31 V8 O20 99.2(3) . . ?
O16 V8 O20 99.9(3) . . ?
O51 V8 O20 148.9(3) . . ?
O31 V8 O22 163.7(3) . 7_565 ?
O16 V8 O22 91.6(3) . 7_565 ?
O51 V8 O22 78.1(2) . 7_565 ?
O20 V8 O22 77.7(3) . 7_565 ?
O31 V8 O25 90.0(3) . . ?
O16 V8 O25 165.3(3) . . ?
O51 V8 O25 77.4(2) . . ?
O20 V8 O25 77.2(2) . . ?
O22 V8 O25 73.6(3) 7_565 . ?
O15 V9 O49 104.6(3) . . ?
O15 V9 O51 100.3(3) . . ?
O49 V9 O51 99.3(3) . . ?
O15 V9 O50 99.4(3) . . ?
O49 V9 O50 99.8(3) . . ?
O51 V9 O50 148.0(3) . . ?
O15 V9 O26 165.1(3) . 7_565 ?
O49 V9 O26 90.3(3) . 7_565 ?
O51 V9 O26 77.5(2) . 7_565 ?
O50 V9 O26 77.0(2) . 7_565 ?
O15 V9 O22 91.3(3) . 7_565 ?
O49 V9 O22 164.1(3) . 7_565 ?
O51 V9 O22 77.3(2) . 7_565 ?
O50 V9 O22 77.3(2) . 7_565 ?
O26 V9 O22 73.7(2) 7_565 7_565 ?
O36 V10 O37 105.1(4) . . ?
O36 V10 O27 98.7(4) . . ?
O37 V10 O27 99.9(3) . . ?
O36 V10 O50 98.7(3) . . ?
O37 V10 O50 100.0(3) . . ?
O27 V10 O50 149.0(3) . . ?
O36 V10 O26 163.1(3) . 7_565 ?
O37 V10 O26 91.8(3) . 7_565 ?
O27 V10 O26 78.2(3) . 7_565 ?
O50 V10 O26 77.6(2) . 7_565 ?
O36 V10 O38 89.3(3) . . ?
O37 V10 O38 165.5(3) . . ?
O27 V10 O38 77.6(2) . . ?
O50 V10 O38 77.1(2) . . ?
O26 V10 O38 73.7(3) 7_565 . ?
O38 V11 O25 179.9(3) . . ?
O38 V11 O26 90.5(3) . . ?
O25 V11 O26 89.4(2) . . ?
O38 V11 O26 90.5(3) . 7_565 ?
O25 V11 O26 89.4(2) . 7_565 ?
O26 V11 O26 90.7(3) . 7_565 ?
O38 V11 O22 90.6(3) . . ?
O25 V11 O22 89.4(2) . . ?
O26 V11 O22 89.6(2) . . ?
O26 V11 O22 178.8(3) 7_565 . ?
O38 V11 O22 90.6(3) . 7_565 ?
O25 V11 O22 89.4(2) . 7_565 ?
O26 V11 O22 178.8(3) . 7_565 ?
O26 V11 O22 89.6(2) 7_565 7_565 ?
O22 V11 O22 90.0(3) . 7_565 ?
O29 V12 O30 104.3(3) . . ?
O29 V12 O51 99.9(3) . . ?
O30 V12 O51 99.8(3) . . ?
O29 V12 O28 98.3(3) . . ?
O30 V12 O28 99.4(3) . . ?
O51 V12 O28 149.2(3) . . ?
O29 V12 O25 165.0(3) . . ?
O30 V12 O25 90.7(3) . . ?
O51 V12 O25 78.4(2) . . ?
O28 V12 O25 77.5(2) . . ?
O29 V12 O26 91.0(3) . 7_565 ?
O30 V12 O26 164.7(3) . 7_565 ?
O51 V12 O26 77.9(2) . 7_565 ?
O28 V12 O26 77.3(3) . 7_565 ?
O25 V12 O26 74.1(3) . 7_565 ?
O39 V13 O39 104.3(4) 7_565 . ?
O39 V13 O27 99.9(3) 7_565 . ?
O39 V13 O27 99.9(3) . . ?
O39 V13 O28 99.1(3) 7_565 . ?
O39 V13 O28 99.1(3) . . ?
O27 V13 O28 148.9(3) . . ?
O39 V13 O26 165.1(3) 7_565 . ?
O39 V13 O26 90.6(3) . . ?
O27 V13 O26 78.0(2) . . ?
O28 V13 O26 77.4(2) . . ?
O39 V13 O26 90.6(3) 7_565 7_565 ?
O39 V13 O26 165.1(3) . 7_565 ?
O27 V13 O26 78.0(2) . 7_565 ?
O28 V13 O26 77.4(2) . 7_565 ?
O26 V13 O26 74.5(3) . 7_565 ?
V1 O1 La1 145.2(5) . . ?
V1 O2 V2 114.0(4) . . ?
V3 O3 V2 114.8(4) . . ?
V4 O4 V3 108.0(4) . . ?
V4 O4 V1 107.2(3) . 5_766 ?
V3 O4 V1 100.7(3) . 5_766 ?
V4 O5 V1 107.1(3) . . ?
V4 O5 V3 106.9(4) . 5_766 ?
V1 O5 V3 100.2(3) . 5_766 ?
V1 O6 V5 114.1(4) . . ?
V3 O7 V5 113.2(4) . . ?
V3 O9 La1 144.2(4) . 5_766 ?
V4 O10 V2 110.8(4) . 5_766 ?
V5 O11 V2 113.4(5) . . ?
V4 O12 V5 109.3(4) . . ?
V7 O14 La1 134.8(3) . . ?
V9 O15 La1 132.8(3) . . ?
V8 O16 La1 134.0(3) . . ?
V7 O20 V8 109.1(3) . . ?
V7 O20 V8 109.1(3) . 7_565 ?
V8 O20 V8 110.2(4) . 7_565 ?
V6 O21 V6 110.5(4) . 7_565 ?
V6 O21 V7 108.4(3) . . ?
V6 O21 V7 108.4(3) 7_565 . ?
V11 O22 V6 97.6(3) . . ?
V11 O22 V8 98.9(3) . 7_565 ?
V6 O22 V8 163.5(3) . 7_565 ?
V11 O22 V7 97.9(2) . . ?
V6 O22 V7 88.5(2) . . ?
V8 O22 V7 88.9(2) 7_565 . ?
V11 O22 V9 98.3(2) . 7_565 ?
V6 O22 V9 89.4(2) . 7_565 ?
V8 O22 V9 88.5(2) 7_565 7_565 ?
V7 O22 V9 163.9(3) . 7_565 ?
V6 O23 La4 135.0(4) . . ?
V6 O24 La1 133.3(3) . 7_565 ?
V11 O25 V12 98.9(3) . 7_565 ?
V11 O25 V12 98.9(3) . . ?
V12 O25 V12 89.5(3) 7_565 . ?
V11 O25 V8 98.1(3) . . ?
V12 O25 V8 163.0(4) 7_565 . ?
V12 O25 V8 88.40(8) . . ?
V11 O25 V8 98.1(3) . 7_565 ?
V12 O25 V8 88.40(8) 7_565 7_565 ?
V12 O25 V8 163.0(4) . 7_565 ?
V8 O25 V8 88.7(3) . 7_565 ?
V11 O26 V10 98.1(3) . 7_565 ?
V11 O26 V12 97.6(3) . 7_565 ?
V10 O26 V12 164.2(3) 7_565 7_565 ?
V11 O26 V9 98.3(2) . 7_565 ?
V10 O26 V9 89.6(2) 7_565 7_565 ?
V12 O26 V9 88.6(2) 7_565 7_565 ?
V11 O26 V13 97.4(2) . . ?
V10 O26 V13 88.5(2) 7_565 . ?
V12 O26 V13 89.0(2) 7_565 . ?
V9 O26 V13 164.3(3) 7_565 . ?
V13 O27 V10 108.6(3) . 7_565 ?
V13 O27 V10 108.6(3) . . ?
V10 O27 V10 109.9(4) 7_565 . ?
V13 O28 V12 110.2(3) . 7_565 ?
V13 O28 V12 110.2(3) . . ?
V12 O28 V12 107.9(4) 7_565 . ?
V12 O29 La3 134.4(4) . 7_565 ?
V12 O30 La2 135.6(3) . . ?
V8 O31 La2 137.1(3) . . ?
V10 O36 La4 135.5(4) . . ?
V10 O37 La3 132.1(4) . 7_565 ?
V11 O38 V6 97.9(3) . . ?
V11 O38 V6 97.9(3) . 7_565 ?
V6 O38 V6 88.3(3) . 7_565 ?
V11 O38 V10 97.6(3) . 7_565 ?
V6 O38 V10 89.37(8) . 7_565 ?
V6 O38 V10 164.5(4) 7_565 7_565 ?
V11 O38 V10 97.6(3) . . ?
V6 O38 V10 164.5(4) . . ?
V6 O38 V10 89.37(8) 7_565 . ?
V10 O38 V10 88.8(3) 7_565 . ?
V13 O39 La3 134.6(3) . . ?
V4 O48 V4 101.4(4) . 5_766 ?
V4 O48 V1 93.7(3) . . ?
V4 O48 V1 93.2(3) 5_766 . ?
V4 O48 V3 93.1(3) . . ?
V4 O48 V3 93.3(3) 5_766 . ?
V1 O48 V3 169.5(4) . . ?
V4 O48 V5 88.3(3) . . ?
V4 O48 V5 170.2(4) 5_766 . ?
V1 O48 V5 86.5(3) . . ?
V3 O48 V5 85.7(2) . . ?
V4 O48 V2 170.9(4) . . ?
V4 O48 V2 87.6(3) 5_766 . ?
V1 O48 V2 86.1(3) . . ?
V3 O48 V2 85.9(2) . . ?
V5 O48 V2 82.6(3) . . ?
V9 O49 La3 133.6(3) . 7_565 ?
V9 O50 V10 108.8(3) . . ?
V9 O50 V6 108.8(3) . 7_565 ?
V10 O50 V6 110.0(3) . 7_565 ?
V12 O51 V8 109.1(3) . . ?
V12 O51 V9 109.7(3) . . ?
V8 O51 V9 109.0(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O6 V1 O1 La1 -103.2(8) . . . . ?
O2 V1 O1 La1 157.7(7) . . . . ?
O5 V1 O1 La1 -11.8(8) . . . . ?
O4 V1 O1 La1 65.3(8) 5_766 . . . ?
V2 V1 O1 La1 161.1(4) . . . . ?
V5 V1 O1 La1 -104.4(8) . . . . ?
V3 V1 O1 La1 27.6(8) 5_766 . . . ?
O1 V1 O2 V2 176.0(5) . . . . ?
O6 V1 O2 V2 71.3(5) . . . . ?
O5 V1 O2 V2 -30.9(12) . . . . ?
O4 V1 O2 V2 -85.3(5) 5_766 . . . ?
O48 V1 O2 V2 -9.2(5) . . . . ?
V5 V1 O2 V2 39.3(4) . . . . ?
V3 V1 O2 V2 -85.8(5) 5_766 . . . ?
O8 V2 O2 V1 -177.7(6) . . . . ?
O11 V2 O2 V1 -72.4(6) . . . . ?
O3 V2 O2 V1 23.0(12) . . . . ?
O10 V2 O2 V1 84.5(5) 5_766 . . . ?
O48 V2 O2 V1 8.8(5) . . . . ?
V5 V2 O2 V1 -39.8(4) . . . . ?
V4 V2 O2 V1 53.6(4) 5_766 . . . ?
V3 V2 O2 V1 8.7(7) . . . . ?
O9 V3 O3 V2 -178.4(5) . . . . ?
O7 V3 O3 V2 -71.2(5) . . . . ?
O4 V3 O3 V2 30.8(12) . . . . ?
O5 V3 O3 V2 85.3(5) 5_766 . . . ?
O48 V3 O3 V2 9.2(5) . . . . ?
V5 V3 O3 V2 -39.3(4) . . . . ?
V1 V3 O3 V2 84.5(5) 5_766 . . . ?
O8 V2 O3 V3 177.5(6) . . . . ?
O11 V2 O3 V3 72.2(5) . . . . ?
O2 V2 O3 V3 -23.2(12) . . . . ?
O10 V2 O3 V3 -84.7(5) 5_766 . . . ?
O48 V2 O3 V3 -9.0(4) . . . . ?
V5 V2 O3 V3 39.8(4) . . . . ?
V1 V2 O3 V3 -8.8(6) . . . . ?
V4 V2 O3 V3 -53.7(4) 5_766 . . . ?
O12 V4 O4 V3 -72.7(4) . . . . ?
O10 V4 O4 V3 179.4(4) . . . . ?
O5 V4 O4 V3 53.1(11) . . . . ?
O48 V4 O4 V3 14.0(4) . . . . ?
O48 V4 O4 V3 93.8(4) 5_766 . . . ?
V5 V4 O4 V3 -34.0(3) . . . . ?
V2 V4 O4 V3 141.9(3) 5_766 . . . ?
O12 V4 O4 V1 179.6(4) . . . 5_766 ?
O10 V4 O4 V1 71.7(4) . . . 5_766 ?
O5 V4 O4 V1 -54.7(11) . . . 5_766 ?
O48 V4 O4 V1 -93.7(4) . . . 5_766 ?
O48 V4 O4 V1 -13.9(3) 5_766 . . 5_766 ?
V5 V4 O4 V1 -141.7(3) . . . 5_766 ?
V2 V4 O4 V1 34.2(3) 5_766 . . 5_766 ?
O1 V1 O6 V5 -178.6(5) . . . . ?
O2 V1 O6 V5 -71.5(5) . . . . ?
O5 V1 O6 V5 85.5(5) . . . . ?
O4 V1 O6 V5 30.6(11) 5_766 . . . ?
O48 V1 O6 V5 9.3(4) . . . . ?
V2 V1 O6 V5 -39.7(4) . . . . ?
V3 V1 O6 V5 85.2(5) 5_766 . . . ?
O13 V5 O6 V1 177.0(5) . . . . ?
O11 V5 O6 V1 72.8(5) . . . . ?
O7 V5 O6 V1 -25.3(11) . . . . ?
O12 V5 O6 V1 -84.4(5) . . . . ?
O48 V5 O6 V1 -9.0(4) . . . . ?
V2 V5 O6 V1 40.2(4) . . . . ?
V4 V5 O6 V1 -53.2(4) . . . . ?
V3 V5 O6 V1 -8.7(6) . . . . ?
O9 V3 O7 V5 175.5(4) . . . . ?
O3 V3 O7 V5 69.8(5) . . . . ?
O4 V3 O7 V5 -85.7(4) . . . . ?
O5 V3 O7 V5 -33.3(12) 5_766 . . . ?
O48 V3 O7 V5 -10.4(4) . . . . ?
V1 V3 O7 V5 -85.8(5) 5_766 . . . ?
V2 V3 O7 V5 38.2(4) . . . . ?
O13 V5 O7 V3 -175.9(5) . . . . ?
O11 V5 O7 V3 -71.3(5) . . . . ?
O6 V5 O7 V3 26.4(11) . . . . ?
O12 V5 O7 V3 85.4(5) . . . . ?
O48 V5 O7 V3 10.1(4) . . . . ?
V2 V5 O7 V3 -38.9(4) . . . . ?
V4 V5 O7 V3 54.2(4) . . . . ?
V1 V5 O7 V3 10.5(6) . . . . ?
O3 V3 O9 La1 -101.7(7) . . . 5_766 ?
O7 V3 O9 La1 158.2(6) . . . 5_766 ?
O4 V3 O9 La1 66.2(7) . . . 5_766 ?
O5 V3 O9 La1 -10.4(7) 5_766 . . 5_766 ?
V5 V3 O9 La1 162.0(4) . . . 5_766 ?
V1 V3 O9 La1 28.0(6) 5_766 . . 5_766 ?
V2 V3 O9 La1 -103.0(7) . . . 5_766 ?
O12 V4 O10 V2 179.7(3) . . . 5_766 ?
O4 V4 O10 V2 -79.8(4) . . . 5_766 ?
O5 V4 O10 V2 80.7(4) . . . 5_766 ?
O48 V4 O10 V2 2.1(15) . . . 5_766 ?
O48 V4 O10 V2 0.2(3) 5_766 . . 5_766 ?
V5 V4 O10 V2 -179.96(16) . . . 5_766 ?
O13 V5 O11 V2 179.3(5) . . . . ?
O6 V5 O11 V2 -77.5(5) . . . . ?
O7 V5 O11 V2 76.8(5) . . . . ?
O12 V5 O11 V2 -2.9(11) . . . . ?
O48 V5 O11 V2 -0.8(4) . . . . ?
V4 V5 O11 V2 -1.0(6) . . . . ?
V3 V5 O11 V2 45.8(4) . . . . ?
V1 V5 O11 V2 -46.6(4) . . . . ?
O8 V2 O11 V5 -178.5(5) . . . . ?
O2 V2 O11 V5 77.6(5) . . . . ?
O3 V2 O11 V5 -76.0(5) . . . . ?
O10 V2 O11 V5 1.0(11) 5_766 . . . ?
O48 V2 O11 V5 0.8(4) . . . . ?
V1 V2 O11 V5 46.6(4) . . . . ?
V4 V2 O11 V5 0.9(6) 5_766 . . . ?
V3 V2 O11 V5 -45.5(4) . . . . ?
O10 V4 O12 V5 179.7(3) . . . . ?
O4 V4 O12 V5 79.4(4) . . . . ?
O5 V4 O12 V5 -80.9(4) . . . . ?
O48 V4 O12 V5 -0.9(3) . . . . ?
O48 V4 O12 V5 -2.1(15) 5_766 . . . ?
V2 V4 O12 V5 -179.99(15) 5_766 . . . ?
O14 V7 O14 La1 178.80(14) 7_565 . . . ?
O20 V7 O14 La1 76.9(5) . . . . ?
O21 V7 O14 La1 -77.9(5) . . . . ?
O22 V7 O14 La1 2.0(14) . . . . ?
O22 V7 O14 La1 -0.3(4) 7_565 . . . ?
O49 V9 O15 La1 -177.7(5) . . . . ?
O51 V9 O15 La1 -75.2(5) . . . . ?
O50 V9 O15 La1 79.5(5) . . . . ?
O26 V9 O15 La1 5.1(15) 7_565 . . . ?
O22 V9 O15 La1 2.2(5) 7_565 . . . ?
O31 V8 O16 La1 -179.1(4) . . . . ?
O51 V8 O16 La1 79.2(4) . . . . ?
O20 V8 O16 La1 -76.8(5) . . . . ?
O22 V8 O16 La1 1.0(4) 7_565 . . . ?
O25 V8 O16 La1 0.7(13) . . . . ?
O24 V6 O23 La4 -179.6(5) . . . . ?
O21 V6 O23 La4 76.5(5) . . . . ?
O50 V6 O23 La4 -78.2(5) 7_565 . . . ?
O22 V6 O23 La4 -3.4(15) . . . . ?
O38 V6 O23 La4 -0.9(5) . . . . ?
O23 V6 O24 La1 -178.2(4) . . . 7_565 ?
O21 V6 O24 La1 -75.7(5) . . . 7_565 ?
O50 V6 O24 La1 80.5(5) 7_565 . . 7_565 ?
O22 V6 O24 La1 2.8(5) . . . 7_565 ?
O38 V6 O24 La1 6.9(14) . . . 7_565 ?
O30 V12 O29 La3 179.0(4) . . . 7_565 ?
O51 V12 O29 La3 -78.1(5) . . . 7_565 ?
O28 V12 O29 La3 77.0(5) . . . 7_565 ?
O25 V12 O29 La3 4.2(14) . . . 7_565 ?
O26 V12 O29 La3 -0.3(5) 7_565 . . 7_565 ?
O29 V12 O30 La2 178.7(4) . . . . ?
O51 V12 O30 La2 75.7(5) . . . . ?
O28 V12 O30 La2 -80.2(5) . . . . ?
O25 V12 O30 La2 -2.7(4) . . . . ?
O26 V12 O30 La2 -4.2(14) 7_565 . . . ?
O16 V8 O31 La2 177.7(4) . . . . ?
O51 V8 O31 La2 -79.5(5) . . . . ?
O20 V8 O31 La2 74.8(5) . . . . ?
O22 V8 O31 La2 -2.9(13) 7_565 . . . ?
O25 V8 O31 La2 -2.3(4) . . . . ?
O37 V10 O36 La4 -179.4(5) . . . . ?
O27 V10 O36 La4 77.8(5) . . . . ?
O50 V10 O36 La4 -76.4(5) . . . . ?
O26 V10 O36 La4 -0.3(14) 7_565 . . . ?
O38 V10 O36 La4 0.5(5) . . . . ?
O36 V10 O37 La3 -178.6(4) . . . 7_565 ?
O27 V10 O37 La3 -76.6(5) . . . 7_565 ?
O50 V10 O37 La3 79.5(5) . . . 7_565 ?
O26 V10 O37 La3 1.7(4) 7_565 . . 7_565 ?
O38 V10 O37 La3 2.1(14) . . . 7_565 ?
O26 V11 O38 V6 89.9(2) . . . . ?
O26 V11 O38 V6 -179.3(2) 7_565 . . . ?
O22 V11 O38 V6 0.3(2) . . . . ?
O22 V11 O38 V6 -89.7(2) 7_565 . . . ?
O26 V11 O38 V6 179.4(2) . . . 7_565 ?
O26 V11 O38 V6 -89.9(2) 7_565 . . 7_565 ?
O22 V11 O38 V6 89.7(2) . . . 7_565 ?
O22 V11 O38 V6 -0.3(2) 7_565 . . 7_565 ?
O26 V11 O38 V10 -0.5(2) . . . 7_565 ?
O26 V11 O38 V10 90.2(2) 7_565 . . 7_565 ?
O22 V11 O38 V10 -90.1(2) . . . 7_565 ?
O22 V11 O38 V10 179.9(2) 7_565 . . 7_565 ?
O26 V11 O38 V10 -90.2(2) . . . . ?
O26 V11 O38 V10 0.5(2) 7_565 . . . ?
O22 V11 O38 V10 -179.9(2) . . . . ?
O22 V11 O38 V10 90.1(2) 7_565 . . . ?
O39 V13 O39 La3 177.67(15) 7_565 . . . ?
O27 V13 O39 La3 -79.4(5) . . . . ?
O28 V13 O39 La3 75.8(5) . . . . ?
O26 V13 O39 La3 -1.5(5) . . . . ?
O26 V13 O39 La3 0.9(15) 7_565 . . . ?
O15 V9 O49 La3 178.8(5) . . . 7_565 ?
O51 V9 O49 La3 75.5(5) . . . 7_565 ?
O50 V9 O49 La3 -78.7(5) . . . 7_565 ?
O26 V9 O49 La3 -1.9(5) 7_565 . . 7_565 ?
O22 V9 O49 La3 -0.9(15) 7_565 . . 7_565 ?

_refine_diff_density_max         3.644
_refine_diff_density_min         -1.649
_refine_diff_density_rms         0.238


